Progress in Polymer Science 46 (2015) 1–24
Contents lists available at ScienceDirect
Progress in Polymer Science journal homepage: www.elsevier.com/locate/ppolysci
Electrospinning of polymer nanoﬁbers for tissue regeneration Tao Jiang a,b,c,∗ , Erica J. Carbone a,b,c , Kevin W.-H. Lo a,b,c,f , Cato T. Laurencin b,c,d,e,f,∗ a
Department of Medicine, Division of Endocrinology, University of Connecticut Health Center, Farmington, CT 06030, USA Institute for Regenerative Engineering, University of Connecticut Health Center, Farmington, CT 06030, USA c Raymond and Beverly Sackler Center for Biological, Physical and Engineering Sciences, University of Connecticut Health Center, Farmington, CT 06030, USA d Department of Orthopaedic Surgery, University of Connecticut Health Center, Farmington, CT 06030, USA e Department of Chemical, Materials and Biomolecular Engineering, University of Connecticut, Storrs, CT 06269, USA f Department of Biomedical Engineering, University of Connecticut, Storrs, CT 06269, USA b
a r t i c l e
i n f o
Article history: Received 11 April 2014 Received in revised form 10 July 2014 Accepted 5 December 2014 Available online 18 December 2014 Keywords: Electrospinning Nanoﬁber Scaffold Musculoskeletal regenerative engineering Growth factor Small molecule
a b s t r a c t Repair and regeneration of human tissues and organs using biomaterials, cells, and/or growth factors is a great challenge for tissue engineers and surgeons. The convergence of advanced materials science, nanotechnology, stem cell science, and developmental biology, which we deﬁne as Regenerative Engineering, represents the next multidisciplinary paradigm to engineer complex tissues. One of the grand challenges in this ﬁeld is to mimic closely the hierarchical architecture and properties of the extracellular matrices (ECM) of the native tissues. A bio-inspired approach to creating biomaterials with nanoscale topographical features, micro- and macroscale gradient structures, and biological domains to interact with target growth factors and cells is key to overcoming this challenge for successful tissue regeneration. Furthermore, the healing and repair of diseased musculoskeletal tissues rely on many signaling pathways, involving numerous growth factors and their receptors. Thus, pharmacological manipulation of the signaling pathways with bioactive molecules is an important component of tissue regeneration. This review summarizes current strategies to develop advanced nanoﬁbrous polymer-based scaffolds via electrospinning, their applications in regenerating human musculoskeletal tissues, and the use of polymer nanoﬁbers to deliver growth factors or small molecules for regenerative medicine. © 2014 Elsevier Ltd. All rights reserved.
Contents 1. 2.
Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Electrospinning polymers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1. Polymer nanoﬁber synthesis via electrospinning . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2. Characterization of nanoﬁbers and nanoﬁbrous scaffolds . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
2 3 3 4
∗ Corresponding authors at: University of Connecticut Health Center, Department of Medicine, Division of Endocrinology, Farmington, CT 06030, USA. Tel.: +1 860 679 7161; fax: +1 860 679 1553 (T. Jiang); University of Connecticut Health Center, Institute for Regenerative Engineering, Farmington, CT 06030, USA. Tel.: +1 860 679 6544; fax: +1 860 679 1255 (C.T. Laurencin). E-mail addresses: [email protected]
(T. Jiang), [email protected]
(C.T. Laurencin). http://dx.doi.org/10.1016/j.progpolymsci.2014.12.001 0079-6700/© 2014 Elsevier Ltd. All rights reserved.
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Advanced nanoﬁbrous scaffolds . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1. Scaffolds comprised of aligned nanoﬁbers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2. Scaffolds comprised of multiphasic micro- or nanoﬁbers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3. Nanoﬁbrous scaffolds with gradients . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4. Nanoﬁbrous scaffolds with superior mechanical properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5. Nanoﬁbrous scaffolds with large pores . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Applications of nanoﬁbers in musculoskeletal regenerative engineering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1. Nanoﬁbers for the regeneration of bone . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2. Nanoﬁbers for the regeneration of soft musculoskeletal tissues . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.1. Cartilage regeneration . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.2. Ligament and tendon regeneration . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.3. Regeneration of soft-to-hard tissue interface . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.4. Nerve regeneration . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.5. Skeletal muscle regeneration . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Nanoﬁber-based delivery of signaling molecules for musculoskeletal tissue regeneration . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1. Growth factor delivery . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2. Small molecule delivery . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Challenges in electrospinning and nanoﬁbrous scaffolds for tissue regeneration . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Conclusions and future outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Acknowledgements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
1. Introduction Musculoskeletal tissue related diseases affect millions of people in the U.S. and worldwide. The repair or regeneration of damaged or diseased musculoskeletal tissues is a major clinical problem, and has been one of the most challenging tasks for orthopedic surgeons. Each year, an estimated 1.5 million bone grafting operations, 650,000 reparative knee procedures, 100,000 anterior cruciate ligament (ACL) reconstructions, and 400,000 shoulder surgeries due to a torn rotator cuff are carried out in the U.S. [1–4]. In these procedures, autografts are considered the gold standards for repair. For example, bone taken from the iliac crest and bone-patella tendon-bone grafts are commonly utilized for bone and ACL repair, respectively. Furthermore, a variety of allografts such as allogenic bone, osteochondral, ligament, and tendon grafts have led to superior clinical outcomes . Although autografts and allografts have been overall successful in repairing musculoskeletal tissues, they suffer from various disadvantages such as limited autograft availability and risk of disease transmission associated with allografts [5,6]. To overcome these problems, tissue engineering, in combination with advanced materials science and stem cell science, has evolved since the early 1990s as a popular research frontier and potential therapy to repair individual tissues and organs . Tissue engineering aims to enhance the repair of living tissues using biomaterials, cells, and growth factors alone, or in combination . Biomaterials, fabricated to mimic the structure and function of tissue-speciﬁc extracellular matrices (ECM), play multiple signiﬁcant roles in cell and tissue ingrowth . Progenitor cells and stem cells, which are capable of differentiating into a multitude of phenotypes, are critical in many cases to compensate for a deﬁciency of normally functional cell populations . Growth factors, typically functioning as signaling molecules by binding to speciﬁc transmembrane receptors on target cells, direct and
5 5 5 7 8 8 10 10 11 11 11 13 13 14 15 15 18 19 19 20 20
regulate numerous cellular processes . In recent years, the importance of convergent research integrating tissue engineering, advanced materials, and stem cells with the seemingly disparate disciplines of physical sciences and developmental biology has been recognized, and a new research direction has been proposed and termed as “regenerative engineering” . While tissue engineering focuses on the ability to repair a speciﬁc tissue, regenerative engineering aims to regenerate or reconstruct complex tissues and biological systems, such as the whole human limb. Advanced materials science, nanotechnology, stem cell science, and developmental biology are important ﬁelds within this new multidisciplinary paradigm to engineer complex tissues. A bio-inspired approach to creating biomaterials with micro- and nanoscale topographical features, macroscale gradient structures, and biological domains to interact with target growth factors and cells is key to successful tissue regeneration. This bio-inspired approach emphasizes fabrication of materials that mimic the unique structures and properties of natural tissues. Furthermore, neo-tissue development and healing of injured musculoskeletal tissues involve many signaling pathways with the participation of a large number of growth factors and signaling molecules. Thus, pharmacological manipulation of these signaling pathways using small molecules is another important component of regenerative engineering . The application of nanoscale materials is crucial in various approaches to regenerating musculoskeletal tissues for several reasons. First, natural musculoskeletal tissues are composed of ﬁnely organized ECM in the nanoscale. For example, natural bone is a nanocomposite material composed mainly of hydroxyapatite nanocrystallites in an organic collagen-rich matrix . The individual, helical collagen chains are 10 nm in length and self-assemble into organized collagen ﬁbers, measuring approximately 500 nm in length. Hydroxyapatite, the mineralized inorganic component of bone, exists as plate-like nanocrystals,
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
measuring 20–80 nm in length. The triple helical structure of collagen gives bone a structural framework with high tensile strength and ﬂexibility, while the nanocrystalline hydroxyapatite provides rigidity and high compressive strength . Second, nanotopographical features, when interacting with cells, have been proven to control and regulate cellular processes as important signaling modalities [15,16]. Nanotopography and local environment inﬂuence trends in cell behavior by providing chemical and physical stimuli to promote cell adhesion, proliferation, morphogenesis, and motility . The provided stimuli include chemical cues and adsorbed protein motifs, as well as the geometry, dimensions, and aspect-ratios of the nanotopographical features [17,18]. ECM materials can be made functional for different musculoskeletal cell types by modifying the stimuli characteristics in order to facilitate cell–matrix interactions at the molecular level. Nanoscale materials can be fabricated into different forms such as nanoparticles, nanoﬁbers, nanospheres, nanotubes, nanogels, nanocapsules, and surfaces with nanotopographical features. These nanostructures can be prepared using a variety of biofabrication methods such as electrospinning, electrospraying, spray drying, phase separation, molecule self-assembly, chemical vapor deposition, and nano-imprinting. Among these nanostructures, nanoﬁbers fabricated from electrospinning are one of the most widely investigated platforms for tissue regeneration . They are characterized by ultra-thin continuous ﬁbers, high surface-to-volume ratio, high porosity, and adjustable pore size distribution. The highly interconnected porous structure of nanoﬁbrous scaffolds provides an appropriate substrate for cell attachment and nutrient transport . In addition, the ECM-mimicking nanoﬁbrous structures have been shown to stimulate in vivo-like organization and morphogenesis of cells in culture . This article ﬁrst provides a concise review of nanoﬁber synthesis by electrospinning, and focuses particularly on the development of various advanced functional nanoﬁbrous scaffolds. Furthermore, this article provides a comprehensive review on the application of these nanoﬁbrous scaffolds in regenerating various musculoskeletal tissues and as delivery vehicles for growth factors and small molecules for musculoskeletal regenerative engineering. 2. Electrospinning polymers 2.1. Polymer nanoﬁber synthesis via electrospinning Electrospinning is a ﬁber-forming process aided by the application of electrostatic forces to control the production of ﬁbers. It is closely related to electrospraying, another well-established method of liquid atomization via electrostatic forces to form droplets. Both electrospinning and electrospraying replace the conventional mechanical forces to form the jet and reduce the size of the ﬁbers or droplets; thus, these processes are also known as electrohydrodynamic jetting [22,23]. Electrospinning ﬁrst appeared in the literature more than a century ago. In 1902, Cooley  and Morton  separately patented methods and apparatuses for electrically dispersing ﬂuids, a concept later known as electrospinning. However, it was not until
the 1990s that electrospun polymer nanoﬁbers became a topic of great research interest [26,27]. Electrospinning is an attractive technique to synthesize nanoﬁbers from various biodegradable polymers due to the simplicity of the technique, ability to effectively control the process, and potential for production scale-up. Fig. 1A illustrates the general set-up of an electrospinning apparatus used to create polymeric nanoﬁbers. The apparatus consists of a high voltage power supply, a syringe and a syringe pump, a needle connected to the syringe, and a metal collector . High electrical potential is applied between the needle and the grounded metal collector. Initially, the polymer solution remains at the tip of the needle due to surface tension. As the electrical potential intensiﬁes, the hemispherical surface of the polymer solution at the needle tip elongates to form a conical shape known as the Taylor cone [28,29]. A further increase of the electrical ﬁeld towards a threshold value causes the formation of a polymer jet as the repulsive electrostatic force overcomes the surface tension. At this point, a polymer jet is ejected from the tip of the Taylor cone and travels rapidly to the metal collector. Before reaching the collector, the jet undergoes a series of electrically driven bending instabilities and gradually thins in air due to elongation and solvent evaporation. The charged jet is eventually collected on a stationary collector (Fig. 1B) and becomes randomly-oriented nanoﬁbers in the form of a non-woven web (Fig. 1C) . Aligned nanoﬁbers can be fabricated by using either a stationary collector with small changes to the collector or different dynamic collectors . In one conﬁguration as shown in Fig. 1D, a rotating drum collector is used at a very high speed to obtain aligned nanoﬁbers (Fig. 1E). A number of processing parameters can be manipulated to ﬁnely tune the diameter and morphology of the nanoﬁbers . First, the properties of the polymer solutions play important roles in determining the electrospinning and electrospraying products. A polymer solution with appropriate viscosity, surface tension, and conductivity is essential to fabricate nanoﬁbers without beads or beads-on-a-string appearance. Whether the polymer jet eventually forms a smooth ﬁber or is dispersed into droplets depends on the polymer’s molecular weight and chain entanglement, as well as the solvent used in the process. If the product of the intrinsic viscosity of the polymer  and polymer concentration c, known as the Berry’s number (Be = c), is greater than a threshold value, small ﬁbers will be produced and the process is termed electrospinning; otherwise, the polymer jet will be disintegrated into droplets and the process is called electrospraying . Speciﬁcally in electrospinning, an increase in viscosity leads to an increase in nanoﬁber diameter, while an increase in the surface tension or conductivity of the polymer solution results in a decrease in nanoﬁber diameter. Second, the electrical potential that provides a suitable level of charge to the polymer solution is also critical to the electrospinning process. A minimum voltage is required for the polymer solution to be ejected from the tip of the Taylor cone. A further increase in voltage decreases the diameter of the nanoﬁbers; however, a high electrical potential is not desired as it may lead to bead formation or defects in the nanoﬁbers . Other processing parameters that
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Fig. 1. (A) Schematic diagram of the electrospinning process. (B) A stationary metal collector. (C) Randomly-oriented nanoﬁbers collected on the stationary collector. (D) A rotating drum collector. (E) Uniaxially aligned nanoﬁbers collected on the rotating drum collector.
affect the diameter, morphology, and orientation of the formed nanoﬁbers include polymer solution feed rate, the inner diameter of the syringe needle, the distance between spinneret and collector, ambient parameters such as temperature and humidity, and the motion of the grounded collector . A number of polymers have been electrospun into nanoﬁbers for tissue engineering applications. Laurencin and co-workers demonstrated that an electrospun nanoﬁbrous structure could serve as a novel scaffold to engineer tissues . This pioneering work has been recently featured as one of the top 25 papers published by the Journal of Biomedical Materials Research over the past 50 years. Laurencin et al. have since investigated a number of electrospun biodegradable nanoﬁbrous scaffolds using polyphosphazenes, poly(lactide-co-glycolide) (PLGA), and poly(caprolactone) (PCL) for wound healing , drug delivery , and regenerating soft [36–42] and hard tissues . Furthermore, polyphosphazene-nanohydroxyapatite composite  and polyphosphazene-PLGA blend  nanoﬁber scaffolds, as well as composite scaffolds comprised of poly(l-lactic acid) (PLLA) nanoﬁbers and sintered microspheres , have been investigated for bone tissue engineering applications. Many research groups have also investigated the electrospinning of a wide range of both natural and synthetic polymers for biomedical engineering applications [20,47]. Some of the well-studied polymers include chitosan [48–51], gelatin [52,53], PCL [54,55], poly(lactic acid) (PLA) [56,57], poly(l-lactide-co-caprolactone) (P(LLA-CL)) [58,59], polyurethane [60,61], and their blends [62–66]. 2.2. Characterization of nanoﬁbers and nanoﬁbrous scaffolds Electrospun nanoﬁbrous scaffolds consist of ultrathin polymer ﬁbers entangled and packed into 3D constructs. Nanoﬁber diameter and orientation, controlled by the electrospinning process, play a key role in the microscopic and macroscopic properties of the nanoﬁbrous scaffolds. These properties include pore size and porosity, as well as mechanical and biological characteristics. Nanoﬁber diameter and orientation are most commonly measured directly by scanning electron microscopy (SEM)
with the aid of image processing software. Typically, a large number of individual nanoﬁbers from different sections of the sample are analyzed using different image analysis software such as Image J, Scion Image, and others [60,67–70]. Nanoﬁber orientation can also be analyzed using these digital-image processing tools. A reference line is drawn along the central orientation and the angular deviations of the oriented nanoﬁbers can be determined. The distribution of ﬁber orientations, ranging from −90◦ to 90◦ where 0◦ is the direction parallel to the reference line, characterizes the degree of alignment of the nanoﬁbers [60,69]. Pore size, pore size distribution, and porosity can be measured by the experimental methods of mercury intrusion porosimetry, liquid extrusion porosimetry, and capillary ﬂow porosimetry. Mercury porosimetry is based on the capillary law governing liquid penetration into small pores, which is expressed by the Washburn equation: D=
4 cos ϕ
where D is pore diameter, P is the applied pressure, is the surface tension, and ϕ is the contact angle. The volume of mercury (V) penetrating the pores is measured directly as a function of applied pressure. This P–V information serves as a unique characterization of pore structure. Liquid extrusion porosimetry and capillary ﬂow porosimetry follow the same rule; however, they use a non-mercury wetting liquid and the liquid is extruded from pores by a nonreacting gas. The differential pressure applied to extrude the liquid and the total volume of the extruded liquid corresponds to the pore size and total pore volume, respectively. Mercury intrusion porosimetry is commonly used on rigid porous scaffolds [71,72], and it has also been used on nanoﬁbrous scaffolds [73,74]. However, mercury intrusion requires very high pressure, which may distort the nanoﬁbrous scaffolds or even lead to sample collapse. Furthermore, the high pressure may reduce pore diameter of the nanoﬁbrous scaffolds [75,76]. In contrast, liquid extrusion porosimetry and capillary ﬂow porosimetry require approximately 5% of the pressure needed for mercury intrusion and produce good resolution of peaks; therefore, they have been widely used as the more appropriate methods to characterize the porous structure of nanoﬁbrous
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
scaffolds [76–79]. In addition to these methods, the porosity of nanoﬁbrous scaffolds can be determined by simple gravimetry following the equations below: Apparent density =
Mass of nanoﬁbrous scaffold Scaffold thickness × scaffold area
Apparent density Bulk material density
It has been shown that the porosity determined by gravimetry is in agreement with the data from a liquid intrusion method , making gravimetry a useful alternative to measure the porosity of nanoﬁbrous scaffolds. 3. Advanced nanoﬁbrous scaffolds Fabrication of scaffolds from nanoﬁbers provides a valuable means to mimic the natural nanoscale ECM of musculoskeletal tissues and provide several key features of the ECM that regulate cell behaviors. As a robust and versatile technique, electrospinning has been applied to produce nanoﬁbers from numerous polymer-based systems, offering opportunities to reconstruct different microenvironments that cells face in vivo. Traditionally, a highly porous, non-woven ﬁbrous mesh with randomly-oriented nanoﬁbers is obtained by collecting the electrospun ﬁbers on a stationary target. This type of nanoﬁber mesh has been widely researched in tissue engineering applications due to the high surface area and greater than 90% porosity. The work has been reviewed in great detail elsewhere [20,81,82]. Recently, with the improved understanding of material structureproperty-function relationships, emphasis has been placed on developing micro- or nano-structures that closely resemble the microenvironments of the native tissues in the body . Speciﬁcally, the development of biomimetic materials mimicking the composition, structure, morphology, and bioactivity of natural tissues represents the future of biomaterials research and development [84,85]. In this regard, the development of advanced nanoﬁbrous scaffolds for regenerative engineering has attracted signiﬁcant research interest and has demonstrated superiority over traditional nanoﬁbrous mesh. 3.1. Scaffolds comprised of aligned nanoﬁbers Many types of musculoskeletal tissues, such as ligament and tendon, are made of collagen ﬁbers with unique anisotropic structures. Therefore, scaffolds with highly ordered nanoﬁbers are advantageous to guide and direct cell proliferation and migration to regenerate these tissues. A number of electrospinning techniques have been successful in producing aligned nanoﬁbrous scaffolds. The most commonly used method involves the use of dynamic rotating collectors. Using a rotating drum collector, researchers have been able to obtain aligned nanoﬁbers from different polymers. It has also been shown that a minimum rotation speed of the mandrel is required for producing aligned nanoﬁbers, and this speed varies among
polymers [86,87]. Other types of rotating collectors, such as a wired drum collector or a rotating collector with sharp edge, have also been successfully used [88,89]. Another approach to fabricating aligned nanoﬁbers is to control the electrospinning jet path by manipulating the external electric ﬁeld. Using a collector comprised of either two separate conductive substrates or a ring collector with a point electrode, Xia and colleagues were able to produce either uniaxially aligned or radially aligned nanoﬁbers [90,91] (Fig. 2A and B). Well-aligned nanoﬁbers can also be obtained by introducing an external magnetic ﬁeld. Yang et al. fabricated arrays of aligned poly(vinyl alcohol) nanoﬁbers by magnetizing the polymer solution with a small amount of magnetic nanoparticles and adding two magnets to the conventional electrospinning setup . More complex, three-dimensional structures made of aligned electrospun nanoﬁbers have also been fabricated. By using two or three pairs of patterned gold electrodes on an insulating substrate as a collector, Li et al. successfully stacked aligned nanoﬁbers into multi-layered ﬁlms, with the orientation of each layer rotated by 90◦ or 60◦  (Fig. 2C). Wang et al. fabricated an electrospun tubular scaffold with circumferentially aligned PLLA nanoﬁbers in the inner surface and a layer of polydimethylsiloxane (PDMS) coating on the outside for enhanced mechanical properties . Wu et al. fabricated three-dimensional PCL nanoﬁbrous tubular scaffolds with both circumferential and axial ﬁber orientations (Fig. 2D) . It has been suggested that multi-directional nanoﬁber orientations can lead to nanoﬁbrous scaffolds with different macroscopic properties. 3.2. Scaffolds comprised of multiphasic micro- or nanoﬁbers The development of biomaterials and devices with precisely controlled and patterned surface/bulk microstructures has attracted great interest from biomedical engineers. First, such microstructures provide a useful platform to study the fundamental cell–cell and cell–biomaterial interactions. Knowledge gained would aid the design of advanced cell–biomaterial constructs for regenerative engineering. Second, ﬁnely tuned microstructures are critical in controlling the spatial distribution and programmable release of encapsulated signaling molecules, as well as guiding the organization of cells and neotissue growth. A variety of multiphasic patterned micro- or nanoﬁbrous structures have been developed via electrospinning and investigated for tissue engineering and drug delivery applications. One type of the micropatterned structures is termed Janus ﬁbers, which contain two distinct phases of hemi-cylinders of a ﬁber with side-by-side compartment conﬁgurations . Recently Lahann et al. developed multicompartmental microparticles, microcylinders, and microﬁbers by applying the side-by-side microﬂuid coﬂow concepts to the electrospraying and electrospinning techniques [97–100]. In the co-jetting process, different polymer solutions are loaded in several side-by-side syringes and pumped together into a common tube to be electrosprayed or electrospun. High solution viscosity and low ﬂow rates ensure a low Reynolds number
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Fig. 2. Aligned nanoﬁbers. (A) Uniaxially aligned nanoﬁbers. (B) Radially aligned poly(-caprolactone) nanoﬁbers on a ring collector. (C) Optical micrograph of a nanoﬁbrous mesh formed by stacking two orthotropic layers of poly(vinyl pyrrolidone) nanoﬁbers. (D) Camera images of the front view and cross section view of a poly(-caprolactone) tubular scaffold made of both axial and circumferentially aligned nanoﬁbers. The insets in (D) show the magniﬁed area of the white boxes. Reproduced with permission from , Copyright 2003, , Copyright 2010, the American Chemical Society, and , Copyright 2010, Springer.
and, thus, a laminar ﬂow that is retained during the electrospraying/electrospinning process. As a result, distinct microcompartments are formed because minimal mass transfer occurs between the different streams of polymer solutions . Lahann and colleagues have demonstrated the formation of a biphasic PLGA-based microﬁbers . By controlling the chemical composition of the polymer in each compartment, a functional azide-peptide sequence was selectively attached either to one side of the Janus ﬁber or to both sides (Fig. 3A and B). NIH3T3 ﬁbroblasts were capable of adhering only to the peptide-modiﬁed ﬁber compartment (Fig. 3C and D), suggesting that the anisotropic bicompartmental microﬁbers could be used for guided cell/tissue growth . Recent advancements in electrospinning have also enabled researchers to fabricate multiphasic nanoﬁbers exhibiting unique core–sheath structure. Coaxial electrospinning was developed as a useful technique to produce core–sheath nanoﬁbers, which have shown great promise in the encapsulation and controlled release of drugs [102,103]. As the core ﬂuid does not need to be electrospinnable, various proteins, growth factors, and genes that might otherwise denature in organic solvents can be dissolved in the core ﬂuid, co-electrospun with the shell solution, and eventually incorporated into the core of the core–sheath structure [104,105]. Rather than
using a core–shell nozzle in the coaxial electrospinning process, one can also fabricate core–sheath nanoﬁbers through emulsion electrospinning using a conventional single-nozzle setup . Core–sheath nanoﬁbers fabricated from both techniques have been successfully used in drug delivery applications, with the beneﬁts of attenuated initial burst release and versatile drug release proﬁles, e.g. dual drug delivery [107–109]. In one study, Wang et al. fabricated core–sheath nanoﬁbers consisting of a Naproxen-containing PCL sheath and a Rhodamine Bcontaining chitosan nanoparticle core (Fig. 3E and F). The core–sheath nanoﬁbers possessed decoupled dual drug release capability and tunable drug release rates, with a higher release rate usually from the drug encapsulated in the nanoﬁber sheath due to shorter diffusional path . More sophisticated multiphasic microﬁbers can be achieved by combining different electrohydrodynamic techniques. Lahann and colleagues have recently reported a novel jetting procedure that combines coaxial electrospinning conventionally used to produce core–sheath ﬁbers with electrohydrodynamic co-jetting used to produce Janus ﬁbers . This approach allowed them to fabricate triphasic or quadriphasic microﬁbers with a Janus core and a polymer shell (Fig. 3G and H). These unique structures may ﬁnd potential uses in drug delivery and regenerative medicine.
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Fig. 3. Biphasic Janus microﬁbers (A–D) fabricated by electrohydrodynamic co-spinning and core–sheath nanoﬁbers (E–F) fabricated by conventional electrospinning show two distinct ﬁber phases. (A) A confocal micrograph shows a bicompartmental Janus ﬁber structure. Only the red ﬂuorescently labeled side of the Janus ﬁber contained acetylene groups, which were further modiﬁed with green ﬂuorescently labeled peptide. (B) Both sides of the Janus ﬁber contained acetylene groups, which were modiﬁed with green ﬂuorescently labeled peptide. Fibroblasts were shown to adhere only to the peptide modiﬁed ﬁber compartment in (C) and to both compartments of the peptide modiﬁed ﬁbers in (D). (E) An SEM micrograph of a core–sheath nanoﬁbrous mesh consisting of a chitosan nanoparticle core and PCL sheath. A small molecule model drug, Rhodamine B, was encapsulated into the chitosan nanoparticles in the core. A second small molecule drug, Naproxen, was incorporated into the nanoﬁber sheath. White arrows indicate the locations of the chitosan nanoparticles. (F) A ﬂuorescent image of ﬂuorescein isothiocyanate (FITC)-conjugated chitosan nanoparticle/PCL core–sheath nanoﬁbers. The green ﬂuorescent dots are chitosan nanoparticles labeled with FITC. (G) An SEM micrograph shows the cross-section of a triphasic microﬁber consisting of a biphasic Janus ﬁber core and PLGA shell. (H) An overlay of confocal and differential interference contrast microscopy images of the ﬁber cross-section shows the two compartments of the Janus core, labeled with green and blue ﬂuorescence, and the PLGA shell. The scale bar stands for 20 m in (A)–(D) and (H), 10 m in (G), and 5 m in (G) inset. Reproduced with permission from , Copyright 2009, , Copyright 2010 John Wiley & Sons Inc, and , Copyright 2013, the American Chemical Society. (For interpretation of the references to color in this ﬁgure legend, the reader is referred to the web version of this article.)
3.3. Nanoﬁbrous scaffolds with gradients Gradient structures are ubiquitously present in the human body, especially within the musculoskeletal tissues. In addition, concentration gradients of signaling molecules play an important role in embryonic development, morphogenesis, angiogenesis, and tissue regeneration [112,113]. Therefore, it has become increasingly popular to develop artiﬁcial matrices with heterogeneous structures and properties for tissue engineering applications. Electrospun nanoﬁbrous scaffolds exhibiting material or structural gradients have been developed to replicate the structures and functions of their natural counterparts. Liu et al. created a mineral-coated PLGA nanoﬁbrous mat by immersing the PLGA mat into simulated body ﬂuid (SBF). A mineral gradient along the long axis of the scaffold was obtained by varying the immersion time in the SBF solution (Fig. 4A) . Using a similar method, Shi et al. fabricated polymethylglutarimide nanoﬁbrous scaffolds with a gradual change in ﬁbronectin content along the long axis. NIH3T3 cells were able to respond to the protein gradient on the scaffold, with more cells spread on the region of higher ﬁbronectin concentration . Scaffolds with a polymer composition gradient can also be achieved by
electrospinning. Du et al. fabricated graded chitosan/PCL blend nanoﬁbrous scaffolds that exhibited chitosan-rich and PCL-rich portions by sequentially co-electrospinning chitosan and PCL solutions (Fig. 4B). Since chitosan is negatively charged and PCL is neutral, negatively charged heparin and heparin-binding vascular endothelial growth factor (VEGF) can be immobilized onto the electrospun scaffolds with a vertical gradient as well . Bottino et al. fabricated a functionally graded membrane by a sequential multilayer electrospinning process . In their study, a spatially designed multilayered nanoﬁbrous membrane was fabricated with a core layer and two functional surface layers that interfaced with bone and epithelial tissues on two sides. In addition to a material gradient, a structural gradient can also be obtained. One approach to creating graded ﬁbrous scaffolds is to combine both nanoﬁbers and microﬁbers into a stratiﬁed architecture. Using sequential electrospinning, Pham et al. fabricated multilayered scaffolds with alternating layers of PCL nanoﬁbers and microﬁbers  (Fig. 4C–F). The layered construct was designed to facilitate cellular inﬁltration into the scaffolds, while simultaneously providing nanoﬁbers as a physical mimicry of ECM. Another approach to fabricating
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Fig. 4. Nanoﬁbrous scaffolds with gradients. (A) Experimental setup for fabricating PLGA nanoﬁbrous scaffolds with a gradient in mineral content (left) and the scanning electron micrographs showing increasing calcium phosphate coating (right, from top to bottom). (B) A graded chitosan/PCL blend nanoﬁbrous scaffold exhibiting chitosan-rich and PCL-rich portions (left: chitosan stained red, PCL stained green). Since heparin binds speciﬁcally to chitosan through ionic interaction and the growth factor VEGF binds to heparin, gradients in bioactive molecules heparin and VEGF can be established (schematic diagram on right). (C) Scanning electron micrographs of multilayered scaffolds with alternating layers of poly(-caprolactone) nanoﬁbers and microﬁbers. (D), (E), and (F) show the magniﬁed images of the corresponding areas in (C). (G) Scanning electron micrograph of random-to-aligned nanoﬁbrous mat. The Fourier Fast Transfer patterns in the inset indicate randomness and alignment of nanoﬁbers on two sides. The scale bar stands for 100 m in (C) and 25 m in (D)–(F). Reproduced with permission from , Copyright 2014, , Copyright 2006,, Copyright 2009, the American Chemical Society and , Copyright 2012, Elsevier Ltd. (For interpretation of the references to color in this ﬁgure legend, the reader is referred to the web version of this article.)
scaffolds with structural gradients is motivated by the stratiﬁed structures of natural tissues. The tendon-to-bone insertion site shows a gradual change in collagen type and collagen ﬁber orientation, from more aligned type I collagen in tendon to more random type II collagen in bone. Xie et al. created an “aligned-to-random” nanoﬁbrous structure to mimic the insertion site using electrospinning equipped with a unique collector composed of two staplershaped metal frames separated by an air gap. Aligned PLGA nanoﬁbers were formed in the air gap, while random nanoﬁbers were formed on the metal frames at both ends [119,120] (Fig. 4G).
nanoﬁbers with diameters ranging from 50 to 500 nm to imitate the dimensions of collagen ﬁbrils in the ECM of natural bone. Biomimetic three-dimensional (3D) scaffolds were then fabricated by rolling the polymer-blend nanoﬁber mat in a concentric manner, creating an open central cavity. This formation replicates the bone marrow cavity as well as the lamellar structure of bone. The polyphosphazene/PLGA nanoﬁber scaffolds showed an average compressive modulus and strength of 151 MPa and 1.5 MPa, respectively, both of which are in the mid-range of human trabecular bone. 3.5. Nanoﬁbrous scaffolds with large pores
3.4. Nanoﬁbrous scaffolds with superior mechanical properties The conventional nanoﬁber mesh usually lacks appropriate mechanical properties to regenerate certain musculoskeletal tissues such as bone. It is critical to match the mechanical properties of the scaffolds with the tissue that they are designed to replace. Therefore, strategies for achieving mechanically competent nanoﬁber-based scaffolds are of great importance. Laurencin and colleagues reported the feasibility of developing a mechanically proﬁcient nanoﬁber matrix using a biomimetic strategy . A miscible polymer blend consisting of a dipeptide-based polyphosphazene and PLGA was electrospun to produce
The electrospun nanoﬁber mesh, though highly porous, usually exhibits dense structure and contains very small pores that may potentially limit cell inﬁltration [121,122]. Therefore, creating nanoﬁbrous scaffolds with appropriate pore size and/or geometry to facilitate cell ingrowth and inﬁltration has attracted research interest in the ﬁeld of regenerative engineering. Several approaches have been used to manipulate the pore size of nanoﬁbrous scaffolds, and thus manipulate cell inﬁltration. Baker et al. prepared aligned PCL/poly(ethylene oxide) (PEO) blend nanoﬁbers by co-electrospinning the two polymers, where PEO served as the sacriﬁcial ﬁber. Improved cellular inﬁltration was achieved by removing the PEO component which increased
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Fig. 5. Strategies to fabricate nanoﬁbrous scaffolds with large pores. (A) A nanoﬁbrous scaffold consisting of “PCL, collagen I, nanoparticulate hydroxyapatite” (stained green), and water-soluble PEO (stained red). (B) Removal of the sacriﬁcial PEO nanoﬁbers led to increase in pore sizes. (C) An electrospun PLLA composite scaffold containing salt particles. (D) A scanning electron micrograph of the scaffold in (C) after the salt leaching/gas forming process, showing the formation of micro-sized pores in the range of 50 – 300 m. (E) A traditional electrospun PCL scaffold with a ﬂat, two-dimensional structure. Inset: SEM of the ﬂat PCL scaffold. (F) A cotton ball-like electrospun PCL scaffold showing a ﬂuffy, three-dimensional structure. Inset: SEM of the cotton ball-like scaffold. Larger pores were observed in the ﬂuffy, three-dimensional scaffold. (G) Electrospun gelatin nanoﬁbrous mesh with nanoﬁber diameter of approximately 110 nm. (H) Electrospun gelatin nanoﬁbrous mesh with a wider nanoﬁber diameter of 600 nm, leading to the formation of larger pores. Reproduced with permission from , Copyright 2012, Elsevier Ltd, , Copyright 2005, Elsevier Ltd, , Copyright 2011, Elsevier Ltd, and , Copyright 2010, John Wiley & Sons Inc. (For interpretation of the references to color in this ﬁgure legend, the reader is referred to the web version of this article.)
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
average pore size and porosity . Phipps et al. fabricated biomimetic electrospun scaffolds consisting of PCL, collagen I, and nanoparticulate hydroxyapatite. They also found that introducing the sacriﬁcial PEO ﬁbers was an effective means to increase scaffold pore size (Fig. 5A and B) . Lee et al. combined electrospinning with a salt leaching/gas forming process to obtain desired pore size. NH4 HCO3 /NaCl salt particles of 150–300 m were sparsely scattered in the interlaminar layers of electrospun nanoﬁber sheets . Micro-sized pores were obtained by removing the salt particles with water, which formed gaseous ammonia and carbon dioxide (Fig. 5C and D). From a different perspective, Blakeney et al. created a low density, uncompressed nanoﬁbrous scaffold using a grounded spherical dish and an array of needle-like probes . Unlike the traditional scaffolds with densely packed nanoﬁbers (Fig. 5E), the uncompressed nanoﬁbrous scaffold had less dense structure and larger pores, which increased cell penetration (Fig. 5F). As an alternative approach, nanoﬁbrous scaffolds with larger pore sizes can be achieved by using ﬁbers with larger diameters (Fig. 5G and H). Both experimental and statistical modeling results have revealed a positive correlation between ﬁber diameter and the pore size of the scaffolds using a variety of polymers [122,127–129]. 4. Applications of nanoﬁbers in musculoskeletal regenerative engineering 4.1. Nanoﬁbers for the regeneration of bone Bone matrix typically makes up more than 90% of the volume of bone tissue, with the remainder made up mostly of cells and blood vessels [130,131]. Bone matrix is a composite material primarily composed of type I collagen ﬁbrils and nanohydroxyapatite. In order to replicate the natural matrix of bone, a variety of synthetic and natural polymers have been combined with hydroxyapatite and electrospun to produce nanoﬁbrous composites as an artiﬁcial ECM for bone repair. Bhattacharyya et al. fabricated poly[bis(ethyl alanato)phosphazene]nanohydroxyapatite composite electrospun nanoﬁbrous scaffolds with a hydroxyapatite content of 50–70%, mimicking the composition of bone tissue . Zhang et al. developed hydroxyapatite/chitosan nanoﬁbrous scaffolds by ﬁrst forming a hydroxyapatite/chitosan nanocomposite suspension in situ and then electrospinning the solution . The composite nanoﬁbrous scaffolds, with 30% hydroxyapatite, were shown to promote the proliferation and mineral deposition of human fetal osteoblasts. Bone is one of the musculoskeletal tissues that have anisotropic structure and mechanical properties. Several techniques have been used to mimic the structural and mechanical anisotropy of bone tissue using electrospun nanoﬁbers. The alignment of ﬁbers has a profound effect on the mechanical properties of the nanoﬁbrous scaffolds. Li et al. showed that a nanoﬁbrous PCL scaffold with aligned ﬁbers had a tensile modulus of 11.6 MPa along the ﬁber direction compared to 2.1 MPa for a non-aligned nanoﬁbrous scaffold . In addition, the prevailing nanoﬁber orientation has been shown to dictate cellular alignment and organization of actin ﬁlaments of human mesenchymal
stem cells. Meng et al. fabricated both randomly-oriented and aligned PLGA/gelatin nanoﬁbrous scaffolds . Compared to the scaffolds with randomly-oriented nanoﬁbers, the aligned nanoﬁbrous scaffolds showed signiﬁcantly increased elastic modulus and tensile strength. The aligned nanoﬁbers guided cell growth along their longitudinal axes, which could be beneﬁcial when utilizing these scaffolds for bone regeneration. Pore size, porosity, and the degree of pore interconnectivity are three key features of tissue-engineered scaffolds that inﬂuence cellular activities. Studies have demonstrated that, while pore sizes of 5–15 m may be appropriate for neovascularization and ﬁbroblast ingrowth, much larger pore sizes of 40–100 m and 100–350 m are required for osteoid ingrowth and for bone regeneration, respectively [134,135]. Although a conventional electrospun nanoﬁbrous scaffold possesses high porosity and excellent pore interconnectivity, the pore size of the scaffold is sub-optimal for regenerating bone, as the small pore size hinders nutrient and oxygen transport, metabolic waste removal, and cellular inﬁltration. Therefore, fabricating a nanoﬁbrous scaffold with larger pore size, without compromising its porosity and pore interconnectivity, has become crucial. Phipps et al. fabricated bone-mimetic electrospun scaffolds consisting of PCL, type I collagen, and nanohydroxyapatite . Three different approaches to increasing the pore size of the scaffolds were investigated including partially digesting collagen I with protease, decreasing the ﬁber packing density, or introducing a sacriﬁcial PEO component. Introduction of the sacriﬁcial PEO polymer was found to be the most effective in increasing pore size. The scaffolds with larger pore sizes signiﬁcantly promoted both mesenchymal stem cell (MSC) and endogenous cell inﬁltration during in vitro cell culture and calvarial organ cultures . The average pore size of ﬁbrous scaffolds increases with an increase in ﬁber diameter as previously mentioned. For instance, the average pore size of an electrospun PCL scaffold reached 45 m from 20 m when the ﬁber diameter was increased to 10 m from 4 m . Traditionally, it has been accepted that nanoﬁbers – due to their large surface area, high aspect ratio, and thus greater protein adsorption – promote cell adhesion and proliferation compared to microﬁbers, raising concerns with using microﬁbers to achieve larger pore sizes. However, the relationship between ﬁber diameter and cellular response has recently been shown to be more complex than originally thought. Several studies have indicated better cell proliferation on microﬁbers than on nanoﬁbers, possibly due to the contact guidance phenomenon where cells are able to extend their lamellipodia along the microﬁlaments and inﬁltrate the larger pores associated with micro-scale ﬁbers [121,136]. Ortiz, Laurencin, and co-workers combined microﬁbrous scaffolds with stem cells and a gene therapy technique, and studied the in vivo ectopic bone formation in immunocompetent mice . PLGA microﬁber mats (ﬁber diameter 4–8 m) were seeded with genetically modiﬁed MSCs expressing recombinant human bone morphogenetic protein-2 (rhBMP-2) and were transplanted into the thigh muscle of C3H/HeN female mice. The results showed that the regenerated bone tissue had similar mineral contents, overall
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
microstructures showing lacunae and canaliculi, chemical compositions, and nanoscale topographical morphologies comparable to the native femoral bone adjacent to the transplantation site . While non-load bearing bone defects can be relatively easily ﬁxed with a wide selection of bone void ﬁller materials, load bearing bone regeneration has presented more challenges to bioengineers and surgeons. It is generally accepted that a scaffold is more biocompatible if it more closely matches the mechanical properties of the native tissue. Inspired by the hierarchical bone structures, Laurencin et al. recently developed a mechanically competent scaffold mimicking both the bone marrow cavity and the lamellar structure of bone (Fig. 6A and B). Electrospun polyphosphazene/PLGA blend nanoﬁbers were oriented in a concentric manner with an open central cavity, creating a biomimetic nanoﬁbrous scaffold . The potential of using this unique spiral scaffold for regenerating bone tissue was evaluated in vitro by monitoring cellular activity and mechanical performance. The polyphosphazene/PLGA blend nanoﬁbers supported the adhesion, proliferation, and phenotype expression of primary rat osteoblasts. In vitro culture demonstrated that the biomimetic scaffolds promoted osteoblast proliferation and differentiation throughout the scaffold architecture, leading to a similar cell–matrix organization to that of native bone (Fig. 6C and D). The blend matrices enhanced cellular activities because the ﬁber diameter and porosity were optimized to provide more surface area for active cellular binding sites and for cell–material interactions. In addition, the scaffold seeded with cells was able to maintain its structural integrity and its initial high compressive modulus throughout the 28-day in vitro culture . This was likely because the mineralized matrix produced by the seeded cells provided structural support to compensate for the loss of integrity due to degradation.
natural polymers, these scaffolds have been shown to support the growth of chondrocytes and the chondrogenic differentiation of stem cells [140–142]. Scaffolds made of aligned nanoﬁbers to mimic the collagen ﬁbril organization of cartilage ECM have been investigated for cartilage repair. Wise et al. created aligned electrospun PCL scaffolds as an artiﬁcial ECM to replicate and regenerate the superﬁcial zone of articular cartilage . Baker et al. fabricated aligned electrospun nanoﬁbrous scaffolds composed of 60% PCL ﬁbers and 40% PEO ﬁbers. The PEO ﬁbers served as a sacriﬁcial component, which led to the formation of macropores after being dissolved from the structure. Unlike typical nanoﬁbrous scaffold systems, in which cell inﬁltration is dramatically limited, the electrospun scaffolds with enlarged pores hastened cell inﬁltration and the scaffold was completely inﬁltrated when cultured with ﬁbrochondrocytes for 9 weeks. However, while ﬁbrochondrocytes proliferated considerably and elaborated a robust collagen- and GAG-rich ECM, human MSCs showed limited division and matrix biosynthesis. This suggested that the 3D microenvironment has crucial control over cell fate processes of different types of cells . Wimpenny et al. proposed a graded composite scaffold by electrospinning poly(l,d-lactic acid) (PLDLA) onto PLDLA microﬁbers rotating at a high speed to achieve nanoﬁber alignment . The beneﬁt of forming a graded composite is to combine the biomimetic architectures of nanoﬁbers with the good mechanical properties of microﬁbers. In addition, the micrometer-size pores due to the presence of the microﬁbers may possibly facilitate cell migration and inﬁltration. The nano-microﬁbrous scaffolds were shown to promote the expression of chondrogenic markers such as type II collagen and aggrecan. This is likely because the size and alignment of the ﬁbers were able to inﬂuence chondrocyte morphology, which is known to inﬂuence gene expression.
4.2. Nanoﬁbers for the regeneration of soft musculoskeletal tissues
4.2.2. Ligament and tendon regeneration One of the most common surgical procedures performed is regeneration or replacement of ruptured/torn ligament or tendon tissues. For example, anterior cruciate ligament (ACL) rupture is one of the most common knee injuries related to disease or trauma. In addition, tendon damage is the most common injury in the young and physically active population . For the past several decades, the use of autografts has been considered the gold standard for ACL reconstruction and tendon regeneration, while allograft tissue has also been commonly used. The use of tissue grafts has a high success rate; however, it is associated with limitations such as donor site pain and morbidity with autografts and potential disease transmission with allografts. Consequently, tissue engineering has become a promising alternative approach for the regeneration of ligament and tendon tissues by using speciﬁcally designed scaffolds, cells, and/or growth factors [147,148]. Electrospun nanoﬁbrous scaffolds have been investigated to repair ligament and tendon by providing an artiﬁcial ECM that mimics the collagen ﬁber bundles present in the natural tissues. In our laboratory, we fabricated an electrospun PLGA nanoﬁbrous scaffold as a novel therapeutic strategy to support and accelerate the
4.2.1. Cartilage regeneration The repair of cartilage defects due to trauma or diseases is another grand challenge for orthopedic surgeons. Articular cartilage is a structurally and functionally complex tissue consisting of highly specialized chondrocytes with various characteristics in different zones. The organization and composition of cartilage ECM vary spatially from the superﬁcial to the deep zones. From the superﬁcial zone to the deep zone of cartilage, the concentration of type II collagen decreases while that of proteoglycan increases . The superﬁcial zone is acellular, consisting of collagen ﬁbrils with a course parallel to the articular surface; while the underneath, middle, and deep zones are formed by a dense, parallel array of collagen ﬁbrils that are oriented perpendicular to the articular surface [138,139]. A calciﬁed cartilage zone separates the deep zone (uncalciﬁed cartilage) from the subchondral bone and is rich in type X collagen . Nanoﬁbrous scaffolds have been used in cartilage tissue engineering due to their structural similarity to the native cartilage ECM. Fabricated from either synthetic or
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Fig. 6. (A) Scanning electron micrograph showing the morphology of a 3D biomimetic nanoﬁbrous scaffold seeded with primary rat osteoblasts and cultured for 28 days. (B) A representative plot of the stress–strain curve of the 3D biomimetic scaffold. The compressive modulus of the scaffold was in the mid-range of human trabecular bone. (C) ECM deposited by the cells bridging the gaps of concentric pattern by 28 days. (D) Immunohistochemical staining for osteopontin, a prominent component of the mineralized ECM, illustrating a homogenous ECM distribution throughout the scaffold after culturing for 28 days. Reproduced with permission from , Copyright 2011, John Wiley & Sons Inc.
healing of a torn rotator cuff . The efﬁcacy of the PLGA nanoﬁbrous scaffold to accelerate the healing rate of a tendon defect was evaluated in an original rodent model. The results showed a signiﬁcant increase in the Young’s modulus for the group that had received augmentation with the nanoﬁbrous scaffold compared to the group that had received only primary supraspinatus repair. In another study, a PLGA nanoﬁbrous scaffold, combined with adipose-derived stem cells and growth/differentiation factor-5 (GDF-5), was evaluated for tendon tissue engineering . Gene expression of the neotendon marker, scleraxis, was upregulated seven- to eightfold at 1 week with GDF-5 treatment when the cells were cultured on the 3D PLGA nanoﬁbrous electrospun scaffold. Expression of scleraxis on the 3D PLGA scaffolds was also signiﬁcantly higher at 2 weeks compared to expression of the marker on 2D PLGA ﬁlms with or without GDF-5 treatment. In addition, expression of the genes that encode type I collagen, the major ECM protein component of tendon tissue, was signiﬁcantly higher for cells on the 3D nanoﬁbrous scaffold than on the 2D ﬁlms irrespective of GDF-5 treatment. The collective effects seen with the 3D-structured scaffold and the GDF-5 treatment suggest that both mechanical and biochemical signals are essential for cellular differentiation on bioengineered scaffolds. Normal healthy tendons are mainly composed of parallel arrays of closely-packed collagen ﬁbers, which leads to highly anisotropic mechanical properties. Therefore,
scaffolds made of aligned nanoﬁbers are attractive candidates in tendon and ligament tissue engineering, as they mimic the anisotropic structure of the native tissues. A number of studies have investigated the effects of nanoﬁber diameter and alignment on the cellular behaviors of both undifferentiated stem cells and committed ﬁbroblasts. Bashur et al. fabricated electrospun polyurethane meshes consisting of either aligned or randomly-oriented nanoﬁbers with diameters in the range of 280 nm to 2.3 m . Bone marrow stromal cells were seeded onto the polymer meshes, and the data suggested that the formation of a ligament-like tissue was enhanced on the surfaces of scaffolds fabricated from aligned submicron ﬁbers. Lee et al. studied the effects of ﬁber alignment and direction of mechanical stimuli on ECM generation by human ligament ﬁbroblasts . Signiﬁcantly more collagen was synthesized on scaffolds with aligned nanoﬁbers than on those with randomly-oriented nanoﬁbers. In addition, the ligament ﬁbroblasts were shown to be more sensitive on the parallel-aligned nanoﬁbers with an externally applied strain in the same direction. Yet in another study, Yin et al. investigated the effect of nanoﬁber alignment on the regulation of tendon stem cell differentiation . Human tendon stem/progenitor cells (hTSPCs) were seeded onto aligned or randomlyoriented poly(l-lactic acid) nanoﬁbers. Aligned nanoﬁbers were shown to increase the expression of tendon-speciﬁc genes compared to randomly-oriented nanoﬁbers in both
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
normal and osteogenic media. In vivo experiments further showed that the aligned nanoﬁbers induced the formation of spindle-shaped cells and tendon-like tissue. On the other hand, randomly-oriented nanoﬁbrous scaffolds induced osteogenesis as evidenced by enhanced alkaline phosphatase activity and alizarin red staining, while the aligned scaffold hindered the osteogenic processes of the hTSPCs. These seemingly contradicting data indicate that aligned nanoﬁbers promote differentiation of tendon stem/progenitor cells into the tenogenic lineage, while randomly-aligned nanoﬁbers promote differentiation into the osteogenic lineage. The topographies of nanoﬁbers have an inﬂuence on cell attachment, orientation, and morphology, which all play roles in determining gene expression. Yin et al. suggest that attachment to the aligned ﬁbers stimulates tenogenic lineage through physical cues and integrin-mediated signaling, since this observation was maintained even in the presence of osteoinductive medium. 4.2.3. Regeneration of soft-to-hard tissue interface The regeneration of the ligament/tendon-to-bone interface remains a challenging task for both scientists and surgeons. Ligament and tendon tissues have complex morphologies at their bone insertion sites, which include zones transitioning from ligament, to stress-distributing ﬁbrocartilage, to calciﬁed cartilage, and then merging into bone. The cells and ECM vary dramatically in these four zones. The ligament/tendon zone consists of ﬁbroblasts, ligament cells, or tenocytes embedded in parallel collagen ﬁbril bundles, primarily made of type I collagen. The ﬁbrocartilage zone is approximately 150 to 400 m in width. The tissue in this zone is primarily composed of collagen type II (typically seen in articular cartilage) with signiﬁcant amounts of aggrecan. The cells are round, aligned in pairs or in rows, and lie in lacunae of the ECM. Separated from the ﬁbrocartilage by a perpendicularly traversing line or tidemark, calciﬁed ﬁbrocartilage ranges from 100 to 300 m in width. Calciﬁed ﬁbrocartilage is primarily composed of collagen type II and large amounts of collagen type X. Collagen ﬁbrils are less aligned in this zone than in the ﬁbrocartilage and ligament zones. In the fourth zone, bone is composed of a highly mineralized collagen type I matrix containing osteoblasts, osteoclasts, and osteocytes. It is clear that the ligament/tendon-to-bone insertion site exhibits gradients in ECM compositions, a gradual increase in mineralization, and a gradual decrease in tissue organization from ligament/tendon to bone [151,152]. To mimic the different collagen ﬁber organizations in both ligament/tendon and bone, Xie et al. created a unique electrospun nanoﬁbrous scaffold with one portion of aligned PLGA nanoﬁbers and a second portion of randomly-oriented nanoﬁbers . The aligned portion of the scaffold was designed to mimic the high level of collagen ﬁber alignment that is responsible for the high tensile modulus and strength in a normal tendon. Meanwhile, the random portion was designed to reproduce the less ordered organization of collagen ﬁbers in bone tissue. Tendon ﬁbroblasts were cultured on the gradient scaffold. The tendon cells on the aligned nanoﬁbers showed a cytoskeleton consisting of actin ﬁlaments aligned with the long axis
of the ﬁbers and produced type I collagen, indicating a high degree of organization. In contrast, the cells on the random nanoﬁbers showed a disorganized actin cytoskeleton and a random distribution of type I collagen . These observations indicate that nanoﬁber alignment can be modiﬁed in order to promote the cellular morphologies naturally present at tendon-to-bone insertion sites. Efforts have also been taken to develop scaffolds that possess continuous compositional gradients as artiﬁcial matrices to regenerate ligament/tendon-to-bone tissue interfaces. To mimic the gradual increase in mineralization, Li et al. fabricated a nanoﬁbrous PLGA mat with a linear gradient of calcium phosphate by electrospinning and a subsequent biomineralization process . The mineral gradient contributed to a gradient in the stiffness and biological functioning of the scaffold. MC3T3 osteoblastic cells preferentially adhered to, and proliferated in, regions with higher calcium phosphate content along the gradated scaffold. Samavedi et al. developed a continuously graded mesh by co-electrospinning nanohydroxyapatite/polycaprolactone and poly(ester urethane) urea elastomer solutions. The nanoﬁber mesh showed gradients in polymer compositions and hydroxyapatite content. The presence of the hydroxyapatite gradient aided in selective mineralization of the nanoﬁbers when soaked in a concentrated simulated body ﬂuid solution, mimicking the ligament-to-bone tissue interface . 4.2.4. Nerve regeneration Peripheral nerve injuries caused by trauma or diseases often necessitate the use of nerve grafts to guide the direction of the axon from the proximal to the distal nerve ends. Currently, an autograft is regarded as the principal method for nerve regeneration; however, it suffers from limited supply, donor site morbidity, and the risk of neuroma formation . Therefore, alternative nerve grafts fabricated from biodegradable polymers in the form of porous scaffolds have attracted research interest and have been evaluated for their efﬁcacy in neural tissue engineering [156–158]. In the development and regeneration of the nervous system, contact guidance has been shown to play an important role in response to an injury in the peripheral nervous system. It has been reported that immature neurons in the medulla oblongata migrate parallel to oriented ﬁbers . Evidence also shows that neurons migrate along tracts of glial cells, or oriented ECM ﬁbers in some instances, during the development of nervous system [160,161]. Since directed growth plays a key role in the regeneration of injured peripheral nerves, a great number of studies have been conducted recently to assess the reaction of neural stem cells, neurons, and glial cells on anisotropic structures carrying topographical cues provided by aligned electrospun nanoﬁbers. Yang el al. seeded neural stem cells on PLLA scaffolds consisting of aligned nanoﬁbers. They observed that the direction of neural stem cell elongation and neurite outgrowth was parallel to the direction of the aligned nanoﬁbers, although the cell growth rate was independent of ﬁber orientation . The importance of nanoﬁber alignment to direct neurite outgrowth and to regenerate nerve defects has been further demonstrated by
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
a number of other studies. Wang et al. evaluated the growth patterns of dorsal root ganglia (DRG) and rat Schwann cells on highly aligned PLLA nanoﬁbrous scaffolds containing crossing ﬁbers. Neurites on these scaffolds were not only directed down the axis of the aligned ﬁbers, but they also grew along the crossed ﬁbers. These crossed ﬁbers sometimes stopped further axonal extension . Kim et al. fabricated both uniaxially and randomly aligned nanoﬁbrous ﬁlms by electrospinning poly(acrylonitrile-comethylacrylate) and seeded the ﬁlms with DRG. In vitro results showed that neurite outgrowth and Schwann cell migration from the DRG extended unidirectionally parallel to the ﬁber alignment, while outgrowth and cell migration was randomly distributed on the random nanoﬁbrous ﬁlms. The ﬁbrous scaffolds were also tested for their ability to regenerate a long, peripheral nerve defect in rats. Interestingly, the aligned, but not the randomly oriented nanoﬁbrous constructs, successfully promoted the regeneration of axons across a 17 mm long nerve gap with the reinnervation of muscles and reformation of neuromuscular junctions . In order to best mimic the hierarchical structures that occur in the mature peripheral nervous system, many studies have focused on developing 3D guidance conduits for nerve regeneration. An ideal nerve conduit should possess a biodegradable and porous channel wall, have the ability to incorporate and deliver signaling molecules and/or supportive cells, and have intraluminal channels to mimic the structure of nerve fascicles . These characteristics would allow the nerve conduits to direct the sprouting of axons from the proximal to the distal ends and reduce the inﬁltration of scar tissue. Electrospun nanoﬁbrous tubular structures consisting of either random nanoﬁbers, aligned nanoﬁbers, or a bilayered structure with aligned nanoﬁbers in the inner layer and random nanoﬁbers in the outer layer have been suggested as potential nerve conduits for nerve regeneration . Wang et al. fabricated tubular chitosan nanoﬁber mesh with or without orientation and bilayered tube with an inner layer of oriented nanoﬁbers and an outer layer of randomized nanoﬁbers (Fig. 7A–C). These tubes were then bridge-grafted into a 10 mm rat sciatic nerve defect. Thirty weeks after implantation, the tube graft with random nanoﬁbers collapsed slightly and the regenerated axons scattered in the loose connective tissue of the lumen, with limited blood vessel formation (Fig. 7D). In contrast, the chitosan tube with oriented nanoﬁbers and the bilayered tube were able to maintain the inner space and form new nerves resembling the isograft. In addition, many large diameter and middle-sized axons matured to mass in the oriented and bilayered tube grafts, respectively (Fig. 7E and F) . The same group demonstrated that incorporation of ␤-tricalcium phosphate particles into the chitosan nanoﬁbrous tube was able to induce electrical polarization and further enhance nerve regeneration . Koh et al. developed a bilayered nerve conduit made out of PLLA nanoﬁbers, which were longitudinally aligned in the lumen and randomly oriented on the outer surface. The construct also contained an intra-luminal guidance channel made of bundles of aligned PLGA nanoﬁbers with encapsulated nerve growth factor. The introduction of the intra-luminal guidance channel increased the mechanical stability of the
nerve conduit and provided a guidance substrate for axonal outgrowth, mimicking the basal lamina structures of the autologous nerve graft. The nerve grafts were evaluated using a rat sciatic nerve defect model. Results showed that functional recovery, as evidenced by muscle reinnervation and withdrawal reﬂex latency, was improved with the use of the nerve construct; however, the axon density was still highest in the autograft group . 4.2.5. Skeletal muscle regeneration Skeletal muscle injuries due to sports-related trauma or other diseases present great challenges in primary care and sports medicine. In major injuries where the muscle structure is irreversibly damaged, surgical interventions such as using autologous tissue to restore muscle functions have been commonly used in the clinic. However, the use of muscle autografts is inevitably limited by tissue availability and donor site morbidity. Therefore, engineered scaffolds mimicking the structure of native muscle tissue may overcome the limitations of muscle autografts and provide a successful option for muscle regeneration. It is well known that functional skeletal tissue consists of highly oriented myoﬁbers derived from multinucleated myotubes, which are formed by the fusion of mononucleated myoblasts . Thus, an artiﬁcial scaffold that guides muscle cell alignment, allowing for oriented myotube formation via topographical and/or chemical cues, is believed to be critical in musculoskeletal myogenesis. Electrospun nanoﬁbrous scaffolds are intrinsically advantageous as artiﬁcial matrices for muscle regeneration. A large number of electrospinnable polymers allows for the screening and selection of a graft material with suitable biological and mechanical properties that match those of skeletal muscle. In addition, the electrospinning process permits the formation of unidirectional nanoﬁbers, which guide the growth of different types of cells. Aligned nanoﬁbrous scaffolds fabricated from both synthetic and natural polymers have been evaluated for skeletal muscle regeneration. Aviss et al. synthesized aligned PLGA nanoﬁbrous scaffolds and evaluated the growth and functions of C2C12 murine myoblasts. The myoblasts not only aligned themselves on the oriented nanoﬁbrous scaffolds, but also produced signiﬁcantly higher expression of the differentiation marker, fast myosin heavy chain, than those on the random nanoﬁbrous scaffolds . Cooper et al. investigated the effect of chitosan-PCL nanoﬁber alignments on the behavior of C2C12 murine myoblasts. It was found that the ﬁber alignment signiﬁcantly enhanced myoblast proliferation and promoted aligned myotube formation in the nanoﬁber orientation. The muscle differentiationspeciﬁc genes, myogenin, troponin T, and myosin heavy chain, were signiﬁcantly up-regulated in muscle cells on the aligned nanoﬁbrous scaffolds compared to the random nanoﬁbrous scaffolds, conﬁrming the ability of aligned chitosan-PCL nanoﬁbers to enhance muscle cell differentiation . In another study, Choi et al. investigated whether electrospun PCL-collagen nanoﬁbers could guide morphogenesis of human skeletal muscle cells and enhance cellular organization. Both the aligned and randomly oriented nanoﬁber meshes were able to maintain the phenotype of the human skeletal muscle cells as
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Fig. 7. Electrospun tubular chitosan nanoﬁbrous scaffolds for nerve regeneration. (A) Non-oriented chitosan nanoﬁber mesh tube. (B) Oriented chitosan nanoﬁber mesh tube. (C) Bilayered chitosan nanoﬁber mesh tube with random ﬁbers in the outer layer and aligned ﬁbers in the inner layer. Insets in (A)–(C) show the orientation of chitosan nanoﬁbers for each tubular structure. (D) Histological image of the non-oriented group showing regenerated axons scattered in the loose connective tissue of the lumen, with some blood vessels of large diameters (V). (E) Many large diameter myelinated axons have matured to mass in the oriented group. (F) Histological image showing a high proﬁle of middle-sized axons in the bilayered group. Scale bars in (D)–(F) stand for 20 m. Reproduced with permission from , Copyright 2008, John Wiley & Sons Inc.
evidenced by the positive immunoﬂuorescent staining of desmin, myosin heavy chain, and sarcomeric actin. The cells and myotubes were arranged along the longitudinal axis of the aligned nanoﬁber direction (Fig. 8E–G), while the myotubes were mostly scattered in all directions on the randomly oriented nanoﬁber meshes (Fig. 8A–C). In addition, the cytoskeletal protein, actin, appeared disordered on the randomly oriented nanoﬁber structures (Fig. 8D); whereas the actin ﬁlaments were well organized along the nanoﬁber direction on the aligned nanoﬁber structures (Fig. 8H). Furthermore, although the nanoﬁber alignment did not affect diameter of the formed myotubes, the average length of the myotubes on the aligned nanoﬁbrous
meshes was more than twice the length of the myotubes on the randomly oriented nanoﬁbrous meshes . 5. Nanoﬁber-based delivery of signaling molecules for musculoskeletal tissue regeneration 5.1. Growth factor delivery During the last several years, musculoskeletal regenerative engineering using electrospun nanoﬁbrous scaffolds combined with growth factors has emerged. These novel scaffolds provide both a biomimetic ECM for cell adhesion and powerful localized signaling moieties, with
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Fig. 8. Immunoﬂuorescent staining images of human skeletal muscle cells on electrospun PCL/collagen nanoﬁber meshes. (A–C) randomly oriented and (E–G) aligned electrospun meshes; (A and E) desmin-positive expression at 3 days after cell seeding, (B and F) myosin heavy chain positive expression at 7 days after cell differentiation, and (C and G) sarcomeric actin-positive expression at 7 days after cell differentiation. Laser confocal microscopy images of F-actin staining on (D) randomly oriented and (H) aligned electrospun PCL/collagen nanoﬁber meshes. Reproduced with permission from , Copyright 2008, Elsevier Ltd.
prolonged biological effects, to direct cellular behaviors [171–174]. Growth factors can be loaded into electrospun nanoﬁbrous scaffolds using a variety of methods, including physical adsorption, covalent linking, and encapsulation (Fig. 9) [171,175,176]. In addition, hydrogels, microparticles, nanoparticles, and other forms of drug delivery devices can be hybridized with nanoﬁbers for speciﬁc biomedical applications [177,178]. However, it should be noted that protein growth factors are easily denatured during the loading process due to the use of harsh organic solvents, cross-linking reagents, low/high pH environments, and high temperatures. Thus, caution must be taken during the incorporation process . Growth factors are usually referred to as large polypeptides that provide the driving forces for many cellular events including proliferation and differentiation . Growth factors also play a dominant role in musculoskeletal tissue regeneration . Therefore, researchers have actively searched for appropriate growth factors to stimulate musculoskeletal regeneration. Today, bone morphogenetic proteins (BMPs) are considered especially important growth factors since these multi-functioning proteins have been shown to be osteoinductive, i.e. they have the capability to induce bone formation in ectopic sites . To date, several devices containing BMP-2 and BMP-7 have been approved by the U.S. Food and Drug Administration for a number of clinical applications including fracture healing, non-union repair, long bone defect repair, spinal fusion, and alveolar ridge and maxillary sinus augmentation [182,183]. BMPs have also been incorporated into polymeric nanoﬁbrous scaffolds for bone tissue regeneration and repair. For instance, the Palleta group
has explored the delivery of BMP-2 within a PLLA based nanoﬁber scaffold for in vivo bone repair and regeneration . They directly incorporated recombinant BMP-2 into a PLLA solution and then electrospun the solution into nanoﬁbers. Their data revealed that the addition of BMP2 signiﬁcantly improved in vivo bone regeneration in a rat critical sized calvarial defect model, therefore showing the efﬁcacy of BMP-2 within the nanoﬁber scaffold. Although the release kinetics of BMP-2 from the scaffold and the mechanism of action were not reported, the PLLA based nanoﬁbers were proposed as efﬁcient carriers of BMP-2 . Given that protein-based growth factors are readily degraded in organic solvents , polymers that are soluble in aqueous-based solutions are favorable for growth factor delivery . For instance, the Kaplan group fabricated a functionalized nanoﬁber scaffold system by incorporating recombinant BMP-2 into silk polyethylene oxide solution. Their results demonstrated that the exogenous BMP-2 could signiﬁcantly enhance the in vitro osteogenic response of human mesenchymal stem cells . In addition to BMPs, other growth factors such as basic ﬁbroblast growth factor (bFGF), vascular endothelial growth factor (VEGF), nerve growth factor (NGF), and platelet-derived growth factor (PDGF) have been introduced into nanoﬁbrous scaffolds to enhance their therapeutic efﬁcacy for musculoskeletal regenerative engineering (Table 1). Casper et al. conducted a study using low molecular weight heparin (LMWH) to incorporate growth factor bFGF onto the surface of poly(ethylene glycol) (PEG) based nanoﬁbers . Their data indicated that LMWH was retained in the nanoﬁbers for at least 14 days, and
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Fig. 9. Schematic representation showing the typical nanoﬁber-based growth factor delivery strategies: (A) physical adsorption; (B) coaxial electrospinning; (C) pore surface immobilization of growth factor-loaded particles; and (D) surface covalent immobilization of growth factors. Reproduced with permission from , Copyright 2012, Elsevier Ltd.
the binding of the bFGF to the PEG-LMWH functionalized nanoﬁbers was found to be stronger than to those functionalized with LMWH alone. This indicates that PEG-LMWH nanoﬁbers could allow for bFGF delivery over the long period of time needed for musculoskeletal regeneration . Apart from regenerating bone tissue, growth factorloaded nanoﬁbrous scaffolds have been shown to inﬂuence the regeneration processes of other musculoskeletal tissues including peripheral nerve, tendon, and skin. Zhang et al. encapsulated NGF into electrospun silk ﬁbroin/P(LLACL)-blended nanoﬁbrous scaffolds. Their data suggested that the NGF released from the nanoﬁbers could effectively promote the regeneration of peripheral nerve in a rat sciatic nerve injury model . Manning et al. developed a novel scaffold system that they claimed is “capable of delivering growth factors and cells in a surgically manageable form for tendon repair” . They incorporated PDGF and adiposederived stem cells (ASCs) into a heparin/ﬁbrin-based hydrogel delivery system and subsequently hybridized the hydrogel with PLGA-based nanoﬁbers. Their data revealed
that delivering PDGF together with ASCs could signiﬁcantly improve tendon healing in a large animal tendon model . Xie et al. recently developed a “dual growth factor releasing nanoparticle-in-nanoﬁber system” for skin regeneration . In their system, PDGF-loaded PLGA nanoparticles were embedded into VEGF-incorporated chitosan/PEO-based electrospun nanoﬁbers. The release proﬁle showed a relatively fast release of VEGF from the nanoﬁbers and a substantial sustained release of PDGF from the nanoparticles. Moreover, their novel scaffold system supported ﬁbroblast growth in vitro, as well as in vivo wound healing in a full thickness rat skin wound model . Although growth factors show potential for use in tissue regeneration and repair, they have various drawbacks. In general, protein instability, high manufacturing cost, and immunogenicity are the common problems associated with protein-based therapeutic strategies. Therefore, new strategies that utilize alternative forms of bioactive factors, such as small bioactive molecules, to obviate these
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
Table 1 Growth factor delivery for musculoskeletal tissue regeneration. Growth factor
Target tissue for regeneration
Physical adsorption onto PCL-based nanoﬁber
Silk ﬁbroin/PEO-blended nanoﬁber
PEG-based nanoﬁber with LMWH Laminin-PCL blend nanoﬁbers
In vitro: human primary osteoblasts In vivo: murine calvarial bone defect repair In vivo: rat critical size calvarial defect repair In vitro: human bone marrow-derived mesenchymal stem cells Not reported
PCL-chitosan nanoﬁbers Silk ﬁbroin/P(LLA-CL)-blended nanoﬁber
Peripheral nerve Peripheral nerve
PDGF-loaded hydrogel embedded in PLGA PDGF-loaded PLGA-based nanoparticles embedded in VEGF-loaded chitosan/PEO-blended nanoﬁber FGF-2-loaded gelatin microspheres incorporated between PCL/PLLA- and PCL/gelatin-blended nanoﬁber layers
In vivo: rat tibial nerve defect repair In vitro: Schwann cells In vitro: PC12 cells In vivo: rat sciatic nerve defect repair In vivo: rat sciatic nerve ligation model In vivo: large animal tendon model In vitro: human dermal ﬁbroblasts In vivo: rat full thickness skin wound repair In vitro: human osteoblasts
PDGF + VEGF
Bone, speciﬁcally at ligament/tendon/cartilageto-bone interfaces
drawbacks have the potential to revolutionize the ﬁeld of musculoskeletal regenerative engineering. 5.2. Small molecule delivery The use of biologically active small molecules is emerging in the area of musculoskeletal regenerative engineering because small molecules do not possess many of the limitations associated with protein-based growth factors, including BMPs [12,182–184,195,196]. For instance, one of the beneﬁts of utilizing small molecules is that they are unlikely to pose a signiﬁcant issue regarding immunogenicity since their molecular sizes are too small to elicit an immune response effectively . In addition, small molecules are often inexpensive and chemically stable when compared to recombinant protein growth factors . It should be noted that the molecular weights of small molecules are less than 1000 Da; therefore, many of them are able to diffuse into cells and interact with speciﬁc intracellular protein receptors. These speciﬁc small molecule-protein interactions can trigger signaling transduction cascades that lead to a desired path of cellular differentiation. For instance, a small molecule could be identiﬁed to activate signaling pathways that stimulate osteoblast-associated gene expression and matrix mineralization, which are processes associated with bone formation . In fact, data from our group and others demonstrated that small molecule cyclic adenosine monophosphate (cAMP) analogs were able to induce
  
in vitro and in vivo bone formation through the Protein Kinase A (PKA)/cAMP response element-binding protein (CREB) signaling mechanism [200–203]. It is also worth noting that the advances in high throughput screening technologies have yielded a large number of other osteoinductive small molecules in the past decade . Taken together, these observations suggest the prospective future of using small molecules for musculoskeletal regenerative engineering, especially for bone tissue repair and reconstruction. While promising, the major concern of using small molecule technologies is the interactions with non-target tissues or organs . Therefore, it is essential to design small molecule delivery systems for tissue regeneration that can effectively localize and sustain controlled release of the small molecule at a speciﬁc site [174,176,184]. Biodegradable nanoﬁber-based polymeric scaffolds have been proposed as controlled drug delivery vehicles of small molecules for regenerating skeletal tissues. For instance, Kouhi et al. incorporated the osteoinductive small molecule simvastatin into electrospun PCL nanoﬁbers and evaluated its potential for bone tissue engineering applications. The drug release kinetics and the in vitro bioactivity were evaluated in simulated body ﬂuids . Their data revealed that the small molecule simvastatin was released in a controlled manner, and a layer of apatite was formed on the nanoﬁber surface . Similarly, Singh et al. incorporated the osteoinductive small molecule resveratrol into PCL nanoﬁbers and evaluated its bioactivity in osteoprogenitor
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
MC3T3-E1 cells . Their results indicated that the resveratrol-loaded PCL nanoﬁber group showed a signiﬁcant increase in mineralized matrix deposition compared to the unloaded control group . However, in vivo studies of osteogenesis in the presence of these small molecule-loaded PCL nanoﬁber scaffolds were not reported in either paper. Recent studies conducted by Das et al. demonstrated that osteoinductive small molecule FTY720loaded nanoﬁbers composed of PCL and PLGA were shown to increase new bone and microvascular formation in a rat mandibular defect model . Speciﬁcally, at week 12 after the implantation, FTY720-loaded nanoﬁber groups demonstrated signiﬁcant new bone formation and new blood vessel formation within the defect area . Taken together, these studies suggest that small molecules in combination with nanoﬁbers have the tremendous potential to revolutionize strategies for bone repair and regeneration. Other than bone tissue, musculoskeletal tissues also include muscles, nerves, cartilage, tendons, joints, and ligaments. Although the utilization of small bioactive molecules for regenerating muscle, cartilage, tendons, and nerves has been reported [12,207], to our knowledge, literature reporting the nanoﬁber-based delivery of small molecules for regenerating these musculoskeletal tissues is very limited. Therefore, further research is needed to investigate the appropriate choice of small molecule, loading and delivery method, dosage requirement, and pre-clinical animal models in order to provide the foundation for future clinical usage in musculoskeletal regeneration. 6. Challenges in electrospinning and nanoﬁbrous scaffolds for tissue regeneration Electrospinning is a convenient and versatile technique to fabricate nanoﬁbers and nanoﬁbrous scaffolds for tissue engineering applications. By altering the polymer solution properties and a number of processing parameters such as voltage, ﬂow rate, distance between the needle tip and the collector, and the type of spinneret and collector, one can fabricate a variety of nanoﬁber assemblies. Nanoﬁbrous structures are highly porous, possess extremely high speciﬁc surface area, and mimic the native microenvironments that cells face in vivo. These attributes make nanoﬁber scaffolds highly advantageous in tissue engineering and drug delivery applications. Nevertheless, challenges remain when applying the electrospinning process and electrospun nanoﬁbrous scaffolds to musculoskeletal tissue regeneration. The main challenge encountered during fabrication is the inability to control ﬁber size and arrangement for optimized cell inﬁltration. Aligned nanoﬁbers are especially ideal for tissue regeneration applications as research has shown that cells tend to elongate, proliferate, and differentiate well along the aligned ﬁbers [56,69,87,133,143,149,162,169,170]. However, methods to obtain a large area of consistent arrangement need to be reﬁned. A rotating drum is the common collector used to create aligned nanoﬁbers, but the rotation speed needs to be ﬁnely adjusted for differences in ﬁber diameter . Increased ﬁber diameter or introduction of a sacriﬁcial polymer component is
often utilized to increase pore size in order to enhance cell inﬁltration [118,121–124,127–129,136,144]; however, increased pore size is also associated with decreased mechanical integrity [209,210]. Another challenge faced when creating nanoﬁbrous scaffolds for musculoskeletal tissue regeneration is the development of suitable mechanical properties. For example, mineral gradients are often introduced to the surfaces of ﬁbers in order to mimic mineralized bone tissue. Unfortunately, the resulting mechanical strength is often not comparable to that of bone. Carefully modifying the ion concentrations of the mineral coating solution can enhance modulus and decreased toughness, providing mechanical properties similar to those of bone tissue . Since polymeric nanoﬁber scaffolds act as temporary templates at sites of tissue regeneration, it is important that the scaffolds maintain this structural integrity for the time needed for cells to inﬁltrate and secrete their own ECM. The issue of scaffold shrinkage during degradation has prompted researchers to fabricate novel patterns of electrospun polymers, such as nestlike-patterned PLGA matrices, to maintain scaffold morphology and strength . Although PLGA is the most widely used polymer for electrospinning nanoﬁbrous scaffolds for tissue regeneration, researchers are exploring other polymer options to provide unique features to suit their desired applications. Since many polymer solutions are not easily spun due to characteristics such as low conductivity and high surface tension, special methods that utilize an electrospinnable carrying solution can be explored to fabricate doublelayered ﬁbers . The carrier layer can be subsequently removed, leaving the desired polymer nanoﬁber intact. Overall, the development of three-dimensional nanoﬁbrous scaffolds that exhibit all of the properties necessary to mimic musculoskeletal tissue and facilitate cell inﬁltration still needs to be optimized for successful application in the clinic. 7. Conclusions and future outlook The emergence of regenerative engineering provides tissue engineers with invaluable tools to achieve the repair and regeneration of musculoskeletal tissues using biomaterials, cells, and growth factors/signaling molecules. In the realm of regenerative engineering, we believe that future research should focus on advanced materials science, stem cells, developmental biology, and strategies to integrate these components into a functional biological system. Creating nanoscale scaffolds with nanotopographical features has been suggested as a key to successfully regenerating musculoskeletal tissues by mimicking the natural microenvironments that cells face in the body. In this review, the use of electrospun nanoﬁbers for musculoskeletal regenerative engineering was discussed. A brief description on the electrospinning process and the parameters of manipulating nanoﬁber properties was provided. Furthermore, the fabrication processes and applications of a number of advanced functional nanoﬁbrous scaffolds were presented. Speciﬁcally, this review discussed anistropic nanoﬁbrous scaffolds made of aligned nanoﬁbers and nanoﬁbrous scaffolds that showed chemical/structural gradients, and/or
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
other macroscopic features to promote cell inﬁltration and mimic natural extracellular matrices. This review also discussed nanoﬁbrous scaffolds that possessed superior mechanical properties for regenerating both hard and soft musculoskeletal tissues. Finally, the use of nanoﬁbers as carriers for growth factors and clinically relevant small molecules for tissue regeneration was discussed. Future research in this highly translational ﬁeld should focus on the convergence of several disciplines including biomimetic nanoﬁbrous scaffold fabrication, stem cells, and manipulation of signaling pathways particularly with small molecules to regenerate complex human tissues and organs. Acknowledgements The authors acknowledge the funding from the National Science Foundation (NSF-EFRI 1332329) and the Presidential Award for Excellence in Science, Engineering, and Math Mentoring (NSF DUE0834313). We also wish to thank the Raymond and Beverly Sackler Center for Biomedical, Biological, Physical and Engineering Sciences Foundation for supporting our Institute. Dr. Laurencin was previously the recipient of a Presidential Faculty Fellow Award from the National Science Foundation. References  Bishop GB, Einhorn TA. Current and future clinical applications of bone morphogenetic proteins in orthopaedic trauma surgery. Int Orthop 2007;31:721–7.  Faulkner A. Usership of regenerative therapies: age, ageing and anti-ageing in the global science and technology of knee cartilage repair. Technol Forecast Soc Change 2015:10, http://dx.doi.org/10.1016/j.techfore.2014.02.020, in press.  Freedman KB, D’Amato MJ, Nedeff DD, Kaz A, Bach BR. Arthroscopic anterior cruciate ligament reconstruction A metaanalysis comparing patellar tendon and hamstring tendon autografts. Am J Sports Med 2003;31:2–11.  Cooper A, Ferraro J, Christensen BA. Recent advancements in soft tissue regeneration. Recent Pat Biomed Eng 2013;6:22–8.  Laurencin CT, Ambrosio A, Borden M, Cooper Jr J. Tissue engineering: orthopedic applications. Annu Rev Biomed Eng 1999;1:19–46.  Laurencin C, Khan Y, El-Amin SF. Bone graft substitutes. Expert Rev Med Devices 2006;3:49–57.  Langer R, Vacanti JP. Tissue engineering. Science 1993;260:920–6.  Spector M. Biomaterials-based tissue engineering and regenerative medicine solutions to musculoskeletal problems. Swiss Med Wkly 2006;136:293–301.  Muschler GF, Nakamoto C, Grifﬁth LG. Engineering principles of clinical cell-based tissue engineering. J Bone Joint Surg 2004;86:1541–58.  Pei M, Seidel J, Vunjak-Novakovic G, Freed L. Growth factors for sequential cellular de-and re-differentiation in tissue engineering. Biochem Biophys Res Commun 2002;294:149–54.  Laurencin CT, Khan Y. Regenerative engineering. Sci Transl Med 2012;4 (160ed9/1-3).  Lo KW-H, Jiang T, Gagnon KA, Nelson C, Laurencin CT. Smallmolecule based musculoskeletal regenerative engineering. Trends Biotechnol 2014;37:74–81.  Rho J-Y, Kuhn-Spearing L, Zioupos P. Mechanical properties and the hierarchical structure of bone. Med Eng Phys 1998;20:92–102.  Laurencin CT, Kumbar SG, Nukavarapu SP. Nanotechnology and orthopedics: a personal perspective. Wiley Interdiscip Rev Nanomed Nanobiotechnol 2009;1:6–10.  Bettinger CJ, Langer R, Borenstein JT. Engineering substrate topography at the micro-and nanoscale to control cell function. Angew Chem Int Ed 2009;48:5406–15.  Li J-R, Shi L, Deng Z, Lo SH, Liu G-y. Nanostructures of designed geometry and functionality enable regulation of cellular signaling processes. Biochemistry 2012;51:5876–93.
 Mendes PM. Cellular nanotechnology: making biological interfaces smarter. Chem Soc Rev 2013;42:9207–18.  Loesberg W, Te Riet J, van Delft F, Schön P, Figdor C, Speller S, van Loon J, Walboomers XF, Jansen JA. The threshold at which substrate nanogroove dimensions may inﬂuence ﬁbroblast alignment and adhesion. Biomaterials 2007;28:3944–51.  Nair LS, Bhattacharyya S, Laurencin CT. Development of novel tissue engineering scaffolds via electrospinning. Expert Opin Biol Ther 2004;4:659–68.  Pham QP, Sharma U, Mikos AG. Electrospinning of polymeric nanoﬁbers for tissue engineering applications: a review. Tissue Eng 2006;12:1197–211.  Schindler M, Ahmed I, Kamal J. A synthetic nanoﬁbrillar matrix promotes in vivo-like organization and morphogenesis for cells in culture. Biomaterials 2005;26:5624–31.  Jaworek A, Sobczyk A. Electrospraying route to nanotechnology: an overview. J Electrostat 2008;66:197–219.  Rutledge GC, Fridrikh SV. Formation of ﬁbers by electrospinning. Adv Drug Deliv Rev 2007;59:1384–91.  Cooley JF. Apparatus for electrically dispersing ﬂuids. US 692631,1902.  Morton WJ. Method of dispersing ﬂuids. US 705691,1902.  Doshi J, Reneker DH. Electrospinning process and applications of electrospun ﬁbers. J Electrostat 1995;35:151–60.  Reneker DH, Chun I. Nanometre diameter ﬁbres of polymer, produced by electrospinning. Nanotechnology 1996;7:216–23.  Taylor G. Disintegration of water drops in an electric ﬁeld. Proc R Soc Lond Ser A 1964;280:383–97.  Yarin AL, Koombhongse S, Reneker DH. Taylor cone and jetting from liquid droplets in electrospinning of nanoﬁbers. J Appl Phys 2001;90:4836–46.  Ramesh Kumar P, Khan N, Vivekanandhan S, Satyanarayana N, Mohanty A, Misra M. Nanoﬁbers: effective generation by electrospinning and their applications. J Nanosci Nanotechnol 2012;12:1–25.  Jaworek A, Krupa A, Lackowski M, Sobczyk A, Czech T, Ramakrishna S, Pliszka D. Nanocomposite fabric formation by electrospinning and electrospraying technologies. J Electrostat 2009;67: 435–8.  Deitzel J, Kleinmeyer J, Harris Dea, Beck Tan N. The effect of processing variables on the morphology of electrospun nanoﬁbers and textiles. Polymer 2001;42:261–72.  Li WJ, Laurencin CT, Caterson EJ, Tuan RS, Ko FK. Electrospun nanoﬁbrous structure: a novel scaffold for tissue engineering. J Biomed Mater Res 2002;60:613–21.  Merrell JG, McLaughlin SW, Tie L, Laurencin CT, Chen AF, Nair LS. Curcumin-loaded poly(-caprolactone) nanoﬁbres: diabetic wound dressing with anti-oxidant and anti-inﬂammatory properties. Clin Exp Pharmacol Physiol 2009;36:1149–56.  Katti DS, Robinson KW, Ko FK, Laurencin CT. Bioresorbable nanoﬁber-based systems for wound healing and drug delivery: optimization of fabrication parameters. J Biomed Mater Res, B 2004;70:286–96.  Kumbar S, James R, Nukavarapu S, Laurencin C. Electrospun nanoﬁber scaffolds: engineering soft tissues. Biomed Mater 2008;3:1–15.  Kumbar SG, Nukavarapu SP, James R, Nair LS, Laurencin CT. Electrospun poly(lactic acid-co-glycolic acid) scaffolds for skin tissue engineering. Biomaterials 2008;29:4100–7.  Taylor ED, Nair LS, Nukavarapu SP, McLaughlin S, Laurencin CT. Novel nanostructured scaffolds as therapeutic replacement options for rotator cuff disease. J Bone Joint Surg 2010;92:170–9.  James R, Kumbar S, Laurencin C, Balian G, Chhabra A. Tendon tissue engineering: adipose-derived stem cell and GDF-5 mediated regeneration using electrospun matrix systems. Biomed Mater 2011;6 (025011/1-26).  James R, Toti U, Laurencin C, Kumbar S. Electrospun nanoﬁbrous scaffolds for engineering soft connective tissues. Methods Mol Biol 2010;726:243–58.  Peach MS, James R, Toti US, Deng M, Morozowich NL, Allcock HR, Laurencin CT, Kumbar SG. Polyphosphazene functionalized polyester ﬁber matrices for tendon tissue engineering: in vitro evaluation with human mesenchymal stem cells. Biomed Mater 2012;7 (045016/1-13).  Peach MS, Kumbar SG, James R, Toti US, Balasubramaniam D, Deng M, Ulery B, Mazzocca AD, McCarthy MB, Morozowich NL, Alcock HR, Laurencin CT. Design and optimization of polyphosphazene functionalized ﬁber matrices for soft tissue regeneration. J Biomed Nanotechnol 2012;8:107–24.
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24  Wang J, Valmikinathan CM, Liu W, Laurencin CT, Yu X. Spiralstructured, nanoﬁbrous, 3D scaffolds for bone tissue engineering. J Biomed Mater Res, A 2010;93:753–62.  Bhattacharyya S, Kumbar SG, Khan YM, Nair LS, Singh A, Krogman NR, Brown PW, Alcock HR, Laurencin CT. Biodegradable polyphosphazene–nanohydroxyapatite composite nanoﬁbers: scaffolds for bone tissue engineering. J Biomed Nanotechnol 2009;5:69–75.  Deng M, Kumbar SG, Nair LS, Weikel AL, Allcock HR, Laurencin CT. Biomimetic structures: biological implications of dipeptidesubstituted polyphosphazene–polyester blend nanoﬁber matrices for load-bearing bone regeneration. Adv Funct Mater 2011;21:2641–51.  Brown JL, Peach MS, Nair LS, Kumbar SG, Laurencin CT. Composite scaffolds: bridging nanoﬁber and microsphere architectures to improve bioactivity of mechanically competent constructs. J Biomed Mater Res, A 2010;95:1150–8.  Huang Z-M, Zhang Y-Z, Kotaki M, Ramakrishna S. A review on polymer nanoﬁbers by electrospinning and their applications in nanocomposites. Compos Sci Technol 2003;63:2223–53.  Zhang Y, Venugopal JR, El-Turki A, Ramakrishna S, Su B, Lim CT. Electrospun biomimetic nanocomposite nanoﬁbers of hydroxyapatite/chitosan for bone tissue engineering. Biomaterials 2008;29:4314–22.  Bhattarai N, Edmondson D, Veiseh O, Matsen FA, Zhang M. Electrospun chitosan-based nanoﬁbers and their cellular compatibility. Biomaterials 2005;26:6176–84.  Geng X, Kwon O-H, Jang J. Electrospinning of chitosan dissolved in concentrated acetic acid solution. Biomaterials 2005;26:5427–32.  Jiang T, Deng M, James R, Nair LS, Laurencin CT. Micro-and nanofabrication of chitosan structures for regenerative engineering. Acta Biomater 2013;10:1632–45.  Li M, Guo Y, Wei Y, MacDiarmid AG, Lelkes PI. Electrospinning polyaniline-contained gelatin nanoﬁbers for tissue engineering applications. Biomaterials 2006;27:2705–15.  Kim HW, Song JH, Kim HE. Nanoﬁber generation of gelatin– hydroxyapatite biomimetics for guided tissue regeneration. Adv Funct Mater 2005;15:1988–94.  Yoshimoto H, Shin Y, Terai H, Vacanti J. A biodegradable nanoﬁber scaffold by electrospinning and its potential for bone tissue engineering. Biomaterials 2003;24:2077–82.  Shin M, Yoshimoto H, Vacanti JP. In vivo bone tissue engineering using mesenchymal stem cells on a novel electrospun nanoﬁbrous scaffold. Tissue Eng 2004;10:33–41.  Yang F, Murugan R, Wang S, Ramakrishna S. Electrospinning of nano/micro scale poly(l-lactic acid) aligned ﬁbers and their potential in neural tissue engineering. Biomaterials 2005;26: 2603–10.  Chen J, Chu B, Hsiao BS. Mineralization of hydroxyapatite in electrospun nanoﬁbrous poly(l-lactic acid) scaffolds. J Biomed Mater Res, A 2006;79:307–17.  Xu C, Inai R, Kotaki M, Ramakrishna S. Aligned biodegradable nanoﬁbrous structure: a potential scaffold for blood vessel engineering. Biomaterials 2004;25:877–86.  Mo X, Xu C, Kotaki Mea, Ramakrishna S. Electrospun P(LLA-CL) nanoﬁber: a biomimetic extracellular matrix for smooth muscle cell and endothelial cell proliferation. Biomaterials 2004;25:1883–90.  Lee CH, Shin HJ, Cho IH, Kang Y-M, Kim I, Park K-D, Shin J-W. Nanoﬁber alignment and direction of mechanical strain affect the ECM production of human ACL ﬁbroblast. Biomaterials 2005;26:1261–70.  Khil MS, Cha DI, Kim HY, Kim IS, Bhattarai N. Electrospun nanoﬁbrous polyurethane membrane as wound dressing. J Biomed Mater Res, B 2003;67:675–9.  Ghasemi-Mobarakeh L, Prabhakaran MP, Morshed M, Nasr-Esfahani M-H, Ramakrishna S. Electrospun poly(caprolactone)/gelatin nanoﬁbrous scaffolds for nerve tissue engineering. Biomaterials 2008;29:4532–9.  Mohammadi Y, Soleimani M, Fallahi-Sichani M, Gazme A, HaddadiAsl V, Areﬁan E, Kiani J, Moradi R, Atashi A, Ahmadbeigi N. Nanoﬁbrous poly(-caprolactone)/poly(vinyl (alcohol)/chitosan hybrid scaffolds for bone tissue engineering using mesenchymal stem cells. Int J Artif Organs 2007;30:204–11.  Dhandayuthapani B, Krishnan UM, Sethuraman S. Fabrication and characterization of chitosan–gelatin blend nanoﬁbers for skin tissue engineering. J Biomed Mater Res, B 2010;94:264–72.  Kai D, Prabhakaran MP, Jin G, Ramakrishna S. Guided orientation of cardiomyocytes on electrospun aligned nanoﬁbers for cardiac tissue engineering. J Biomed Mater Res, B 2011;98:379–86.
 Kim HW, Yu HS, Lee HH. Nanoﬁbrous matrices of poly(lactic acid) and gelatin polymeric blends for the improvement of cellular responses. J Biomed Mater Res, A 2008;87:25–32.  Christopherson GT, Song H, Mao HQ. The inﬂuence of ﬁber diameter of electrospun substrates on neural stem cell differentiation and proliferation. Biomaterials 2009;30:556–64.  Venugopal J, Ma L, Yong T, Ramakrishna S. In vitro study of smooth muscle cells on polycaprolactone and collagen nanoﬁbrous matrices. Cell Biol Int 2005;29:861–7.  Wang HB, Mullins ME, Cregg JM, Hurtado A, Oudega M, Trombley MT, Gilbert RJ. Creation of highly aligned electrospun poly-l-lactic acid ﬁbers for nerve regeneration applications. J Neural Eng 2009;6 (016001/1-15).  Wang C-Y, Zhang K-H, Fan C-Y, Mo X-M, Ruan HJ, Li FF. Aligned natural–synthetic polyblend nanoﬁbers for peripheral nerve regeneration. Acta Biomater 2011;7:634–43.  Jiang T, Abdel-Fattah WI, Laurencin CT. In vitro evaluation of chitosan/poly(lactic acid-glycolic acid) sintered microsphere scaffolds for bone tissue engineering. Biomaterials 2006;27:4894–903.  Jiang T, Khan Y, Nair LS, Abdel-Fattah WI, Laurencin CT. Functionalization of chitosan/poly(lactic acid-glycolic acid) sintered microsphere scaffolds via surface heparinization for bone tissue engineering. J Biomed Mater Res, A 2010;93:1193–208.  Lowery JL, Datta N, Rutledge GC. Effect of ﬁber diameter, pore size and seeding method on growth of human dermal ﬁbroblasts in electrospun poly(-caprolactone) ﬁbrous mats. Biomaterials 2010;31:491–504.  Min B-M, Lee G, Kim SH, Nam YS, Lee TS, Park WH. Electrospinning of silk ﬁbroin nanoﬁbers and its effect on the adhesion and spreading of normal human keratinocytes and ﬁbroblasts in vitro. Biomaterials 2004;25:1289–97.  Ziabari M, Mottaghitalab V, Haghi AK. Evaluation of electrospun nanoﬁber pore structure parameters. Kor J Chem Eng 2008;25:923–32.  Jena A, Gupta K. Pore volume of nanoﬁber nonwovens. Int Nonwovens J 2005;14:25–30.  Frey MW, Li L. Electrospinning and porosity measurements of nylon-6/poly(ethylene oxide) blended non-wovens. J Eng Fibers Fabrics 2007;2:31–7.  Gupta D, Venugopal J, Prabhakaran MP, Dev V, Low S, Choon AT, Ramakrishna S. Aligned and random nanoﬁbrous substrate for the in vitro culture of Schwann cells for neural tissue engineering. Acta Biomater 2009;5:2560–9.  Li D, Frey MW, Joo YL. Characterization of nanoﬁbrous membranes with capillary ﬂow porometry. J Memb Sci 2006;286:104–14.  Soliman S, Pagliari S, Rinaldi A, Forte G, Fiaccavento R, Pagliari F, Franzese O, Minieri M, Di Nardo P, Licoccia S, Traversa E. Multiscale three-dimensional scaffolds for soft tissue engineering via multimodal electrospinning. Acta Biomater 2010;6:1227–37.  Vasita R, Katti DS. Nanoﬁbers and their applications in tissue engineering. Int J Nanomed 2006;1:15–30.  Ma Z, Kotaki M, Inai R, Ramakrishna S. Potential of nanoﬁber matrix as tissue-engineering scaffolds. Tissue Eng 2005;11:101–9.  Langer R, Tirrell DA. Designing materials for biology and medicine. Nature 2004;428:487–92.  Langer R, Peppas NA. Advances in biomaterials, drug delivery, and bionanotechnology. AIChE J 2004;49:2990–3006.  Rice JJ, Martino MM, De Laporte L, Tortelli F, Briquez PS, Hubbell JA. Engineering the regenerative microenvironment with biomaterials. Adv Healthc Mater 2012;2:57–71.  Matthews JA, Wnek GE, Simpson DG, Bowlin GL. Electrospinning of collagen nanoﬁbers. Biomacromolecules 2002;3:232–8.  Choi JS, Lee SJ, Christ GJ, Atala A, Yoo JJ. The inﬂuence of electrospun aligned poly(-caprolactone)/collagen nanoﬁber meshes on the formation of self-aligned skeletal muscle myotubes. Biomaterials 2008;29:2899–906.  Katta P, Alessandro M, Ramsier R, Chase G. Continuous electrospinning of aligned polymer nanoﬁbers onto a wire drum collector. Nano Lett 2004;4:2215–8.  Theron A, Zussman E, Yarin A. Electrostatic ﬁeld-assisted alignment of electrospun nanoﬁbres. Nanotechnology 2001;12:384–90.  Li D, Wang Y, Xia Y. Electrospinning of polymeric and ceramic nanoﬁbers as uniaxially aligned arrays. Nano Lett 2003;3:1167–71.  Xie J, MacEwan MR, Ray WZ, Liu W, Siewe DY, Xia Y. Radially aligned, electrospun nanoﬁbers as dural substitutes for wound closure and tissue regeneration applications. ACS Nano 2010;4:5027–36.  Yang D, Lu B, Zhao Y, Jiang X. Fabrication of aligned ﬁbrous arrays by magnetic electrospinning. Adv Mater 2007;19:3702–6.
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
 Li D, Wang Y, Xia Y. Electrospinning nanoﬁbers as uniaxially aligned arrays and layer-by-layer stacked ﬁlms. Adv Mater 2004;16: 361–6.  Wang Y, Shi H, Qiao J, Tian Y, Wu M, Zhang W, Lin Y, Niu Z, Huang Y. Electrospun tubular scaffold with circumferentially aligned nanoﬁbers for regulating smooth muscle cell growth. ACS Appl Mater Interfaces 2014;6:2958–62.  Wu H, Fan J, Chu C-C, Wu J. Electrospinning of small diameter 3-D nanoﬁbrous tubular scaffolds with controllable nanoﬁber orientations for vascular grafts. J Mater Sci Mater Med 2010;21:3207–15.  George MC, Braun PV. Multicompartmental materials by electrohydrodynamic cojetting. Angew Chem Int Ed 2009;48: 8606–9.  Yoshida M, Roh KH, Mandal S, Bhaskar S, Lim D, Nandivada H, Deng X, Lahann J. Structurally controlled bio-hybrid materials based on unidirectional association of anisotropic microparticles with human endothelial cells. Adv Mater 2009;21:4920–5.  Roh K-H, Martin DC, Lahann J. Biphasic Janus particles with nanoscale anisotropy. Nat Mater 2005;4:759–63.  Bhaskar S, Hitt J, Chang SWL, Lahann J. Multicompartmental microcylinders. Angew Chem Int Ed 2009;48:4589–93.  Bhaskar S, Lahann J. Microstructured materials based on multicompartmental ﬁbers. J Am Chem Soc 2009;131:6650–1.  Mandal S, Bhaskar S, Lahann J. Micropatterned ﬁber scaffolds for spatially controlled cell adhesion. Macromol Rapid Commun 2009;30:1638–44.  Jiang Y-N, Mo H-Y, Yu D-G. Electrospun drug-loaded core–sheath PVP/zein nanoﬁbers for biphasic drug release. Int J Pharm 2012;438:232–9.  Liao I, Chew S, Leong K. Aligned core–shell nanoﬁbers delivering bioactive proteins. Nanomedicine 2006;1:465–71.  Liao I, Chen S, Liu JB, Leong KW. Sustained viral gene delivery through core–shell ﬁbers. J Controlled Release 2009;139:48–55.  Yan S, Xiaoqiang L, Lianjiang T, Chen H, Xiumei M. Poly(l-lactideco--caprolactone) electrospun nanoﬁbers for encapsulating and sustained releasing proteins. Polymer 2009;50:4212–9.  Xu X, Zhuang X, Chen X, Wang X, Yang L, Jing X. Preparation of core–sheath composite nanoﬁbers by emulsion electrospinning. Macromol Rapid Commun 2006;27:1637–42.  Yu D-G, Chian W, Wang X, Li X-Y, Li Y, Liao Y-Z. Linear drug release membrane prepared by a modiﬁed coaxial electrospinning process. J Memb Sci 2013;428:150–6.  Yang Y, Xia T, Zhi W, Wei L, Weng J, Zhang C, Li X. Promotion of skin regeneration in diabetic rats by electrospun core–sheath ﬁbers loaded with basic ﬁbroblast growth factor. Biomaterials 2011;32:4243–54.  Jo E, Lee S, Kim KT, Won YS, Kim HS, Cho EC, Jeong U. Core–sheath nanoﬁbers containing colloidal arrays in the core for programmable multi-agent delivery. Adv Mater 2009;21:968–72.  Wang Y, Qiao W, Yin T. A novel controlled release drug delivery system for multiple drugs based on electrospun nanoﬁbers containing nanoparticles. J Pharm Sci 2010;99:4805–11.  Lee KJ, Park T-H, Hwang S, Yoon J, Lahann J. Janus-core and shell microﬁbers. Langmuir 2013;29:6181–6.  Liu A, Niswander LA. Bone morphogenetic protein signalling and vertebrate nervous system development. Nat Rev Neurosci 2005;6:945–54.  Adams RH, Alitalo K. Molecular regulation of angiogenesis and lymphangiogenesis. Nat Rev Mol Cell Biol 2007;8:464–78.  Liu W, Lipner J, Xie J, Manning CN, Thomopoulos S, Xia Y. Nanoﬁber scaffolds with gradients in mineral content for spatial control of osteogenesis. ACS Appl Mater Interfaces 2014;6:2842–9.  Shi J, Wang L, Zhang F, Li H, Lei L, Liu L, Chen Y. Incorporating protein gradient into electrospun nanoﬁbers as scaffolds for tissue engineering. ACS Appl Mater Interfaces 2010;2:1025–30.  Du F, Wang H, Zhao W, Li D, Kong D, Yang J, Zhang Y. Gradient nanoﬁbrous chitosan/poly -caprolactone scaffolds as extracellular microenvironments for vascular tissue engineering. Biomaterials 2012;33:762–70.  Bottino MC, Thomas V, Janowski GM. A novel spatially designed and functionally graded electrospun membrane for periodontal regeneration. Acta Biomater 2011;7:216–24.  Pham QP, Sharma U, Mikos AG. Electrospun poly(-caprolactone) microﬁber and multilayer nanoﬁber/microﬁber scaffolds: characterization of scaffolds and measurement of cellular inﬁltration. Biomacromolecules 2006;7:2796–805.  Xie J, Li X, Lipner J, Manning CN, Schwartz AG, Thomopoulos S, Xia Y. Aligned-to-random” nanoﬁber scaffolds for mimicking the structure of the tendon-to-bone insertion site. Nanoscale 2010;2:923–6.
 Xie J, MacEwan MR, Li X, Sakiyama-Elbert SE, Xia Y. Neurite outgrowth on nanoﬁber scaffolds with different orders, structures, and surface properties. ACS Nano 2009;3:1151–9.  Chen M, Patra PK, Warner SB, Bhowmick S. Role of ﬁber diameter in adhesion and proliferation of NIH 3T3 ﬁbroblast on electrospun polycaprolactone scaffolds. Tissue Eng 2007;13:579–87.  Sisson K, Zhang C, Farach-Carson MC, Chase DB, Rabolt JF. Fiber diameters control osteoblastic cell migration and differentiation in electrospun gelatin. J Biomed Mater Res, A 2010;94:1312–20.  Baker BM, Gee AO, Metter RB, Nathan AS, Marklein RA, Burdick JA, Mauck RL. The potential to improve cell inﬁltration in composite ﬁber-aligned electrospun scaffolds by the selective removal of sacriﬁcial ﬁbers. Biomaterials 2008;29:2348–58.  Phipps MC, Clem WC, Grunda JM, Clines GA, Bellis SL. Increasing the pore sizes of bone-mimetic electrospun scaffolds comprised of polycaprolactone, collagen I and hydroxyapatite to enhance cell inﬁltration. Biomaterials 2012;33:524–34.  Lee YH, Lee JH, An I-G, Kim C, Lee DS, Lee YK, Nam J-D. Electrospun dual-porosity structure and biodegradation morphology of Montmorillonite reinforced PLLA nanocomposite scaffolds. Biomaterials 2005;26:3165–72.  Blakeney BA, Tambralli A, Anderson JM, Andukuri A, Lim D-J, Dean DR, Jun H-W. Cell inﬁltration and growth in a low density, uncompressed three-dimensional electrospun nanoﬁbrous scaffold. Biomaterials 2011;32:1583–90.  Rnjak-Kovacina J, Wise SG, Li Z, Maitz PK, Young CJ, Wang Y, Weiss AS. Tailoring the porosity and pore size of electrospun synthetic human elastin scaffolds for dermal tissue engineering. Biomaterials 2011;32:6729–36.  Balguid A, Mol A, van Marion MH, Bank RA, Bouten CV, Baaijens FP. Tailoring ﬁber diameter in electrospun poly(-caprolactone) scaffolds for optimal cellular inﬁltration in cardiovascular tissue engineering. Tissue Eng, A 2008;15:437–44.  Eichhorn SJ, Sampson WW. Statistical geometry of pores and statistics of porous nanoﬁbrous assemblies. J R Soc Interface 2005;2:309–18.  Ross MH, Kaye GI, Pawlina W, Histology:. A text and atlas. Philadelphia, PA: Lippincott Williams & Wilkins; 2003. p. 201–37.  Bilezikian JP, Raisz LG, Rodan GA. Principles of bone biology. San Diego, CA: Academic Press; 1996. p. 3–14.  Li W-J, Mauck RL, Cooper JA, Yuan X, Tuan RS. Engineering controllable anisotropy in electrospun biodegradable nanoﬁbrous scaffolds for musculoskeletal tissue engineering. J Biomechanics 2007;40:1686–93.  Meng Z, Wang Y, Ma C, Zheng W, Li L, Zheng Y. Electrospinning of PLGA/gelatin randomly-oriented and aligned nanoﬁbers as potential scaffold in tissue engineering. Mater Sci Eng C 2010;30:1204–10.  Yang S, Leong K-F, Du Z, Chua C-K. The design of scaffolds for use in tissue engineering. Part I. Traditional factors. Tissue Eng 2001;7:679–89.  Whang K, Healy K, Elenz D, Nam E, Tsai D, Thomas C, Nuber GW, Glorieux FH, Travers R, Sprague SM. Engineering bone regeneration with bioabsorbable scaffolds with novel microarchitecture. Tissue Eng 1999;5:35–51.  Badami AS, Kreke MR, Thompson MS, Rifﬂe JS, Goldstein AS. Effect of ﬁber diameter on spreading, proliferation, and differentiation of osteoblastic cells on electrospun poly(lactic acid) substrates. Biomaterials 2006;27:596–606.  Pelled G, Tai K, Sheyn D, Zilberman Y, Kumbar S, Nair LS, Laurencin CT, Gazit D, Ortiz C. Structural and nanoindentation studies of stem cell-based tissue-engineered bone. J Biomech 2007;40: 399–411.  Teshima R, Otsuka T, Takasu N, Yamagata N, Yamamoto K. Structure of the most superﬁcial layer of articular cartilage. J Bone Joint Surg Br 1995;77:460–4.  Ap Gwynn I, Wade S, Ito K, Richards R. Novel aspects to the structure of rabbit articular cartilage. Eur Cell Mater 2002;4:18–29.  Subramanian A, Vu D, Larsen GF, Lin H-Y. Preparation and evaluation of the electrospun chitosan/PEO ﬁbers for potential applications in cartilage tissue engineering. J Biomater Sci Polym Ed 2005;16:861–73.  Shin HJ, Lee CH, Cho IH, Kim Y-J, Lee Y-J, Kim IA, Park KD, Yui N, Shin JW. Electrospun PLGA nanoﬁber scaffolds for articular cartilage reconstruction: mechanical stability, degradation and cellular responses under mechanical stimulation in vitro. J Biomater Sci Polym Ed 2006;17:103–19.  Alves da Silva M, Martins A, Costa-Pinto A, Costa P, Faria S, Gomes M, Reis RL, Neves NM. Cartilage tissue engineering using
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24
electrospun PCL nanoﬁber meshes and MSCs. Biomacromolecules 2010;11:3228–36. Wise JK, Yarin AL, Megaridis CM, Cho M. Chondrogenic differentiation of human mesenchymal stem cells on oriented nanoﬁbrous scaffolds: engineering the superﬁcial zone of articular cartilage. Tissue Eng, A 2008;15:913–21. Baker BM, Nathan AS, Gee AO, Mauck RL. The inﬂuence of an aligned nanoﬁbrous topography on human mesenchymal stem cell ﬁbrochondrogenesis. Biomaterials 2010;31:6190–200. Wimpenny I, Ashammakhi N, Yang Y. Chondrogenic potential of electrospun nanoﬁbres for cartilage tissue engineering. J Tissue Eng Regen Med 2012;6:536–49. Järvinen TA, Kannus P, Paavola M, Järvinen TL, Józsa L, Järvinen M. Achilles tendon injuries. Curr Opin Rheumatol 2001;13:150–5. Petrigliano FA, McAllister DR, Wu BM. Tissue engineering for anterior cruciate ligament reconstruction: a review of current strategies. Arthroscopy 2006;22:441–51. Jiang T, Deng M, Abdel-Fattah WI, Laurencin CT. Chitosan-based biopharmaceutical scaffolds in tissue engineering and regenerative medicine. In: Sarmento B, Das Neves J, editors. Chitosan-based systems for biopharmaceuticals: delivery, targeting and polymer therapeutics. West Sussex: John Wiley & Sons Inc; 2012. p. 393–427. Bashur CA, Shaffer RD, Dahlgren LA, Guelcher SA, Goldstein AS. Effect of ﬁber diameter and alignment of electrospun polyurethane meshes on mesenchymal progenitor cells. Tissue Eng, A 2009;15:2435–45. Yin Z, Chen X, Chen JL, Shen WL, Hieu Nguyen TM, Gao L, Ouyang HW. The regulation of tendon stem cell differentiation by the alignment of nanoﬁbers. Biomaterials 2010;31:2163–75. Doschak M, Zernicke R. Structure, function and adaptation of bonetendon and bone-ligament complexes. J Musculoskelet Neuronal Interact 2005;5:35–40. Yang PJ, Temenoff JS. Engineering orthopedic tissue interfaces. Tissue Eng, B 2009;15:127–41. Li X, Xie J, Lipner J, Yuan X, Thomopoulos S, Xia Y. Nanoﬁber scaffolds with gradations in mineral content for mimicking the tendon-to-bone insertion site. Nano Lett 2009;9:2763–8. Samavedi S, Olsen Horton C, Guelcher SA, Goldstein AS, Whittington AR. Fabrication of a model continuously graded co-electrospun mesh for regeneration of the ligament–bone interface. Acta Biomater 2011;7:4131–8. Mackinnon SE, Hudson AR. Clinical application of peripheral nerve transplantation. Plast Reconstr Surg 1992;90:695–9. Subramanian A, Krishnan UM, Sethuraman S. Development of biomaterial scaffold for nerve tissue engineering: biomaterial mediated neural regeneration. J Biomed Sci 2009;16 (108/1-11). Hadlock T, Sundback C, Hunter D, Cheney M, Vacanti JP. A polymer foam conduit seeded with Schwann cells promotes guided peripheral nerve regeneration. Tissue Eng 2000;6:119–27. Bini T, Gao S, Xu X, Wang S, Ramakrishna S, Leong K. Peripheral nerve regeneration by microbraided poly(l-lactide-coglycolide) biodegradable polymer ﬁbers. J Biomed Mater Res, A 2004;68:286–95. Ono K, Kawamura K. Migration of immature neurons along tangentially oriented ﬁbers in the subpial part of the fetal mouse medulla oblongata. Exp Brain Res 1989;78:290–300. Nadarajah B, Alifragis P, Wong RO, Parnavelas JG. Ventricledirected migration in the developing cerebral cortex. Nat Neurosci 2002;5:218–24. O’Rourke NA, Sullivan DP, Kaznowski CE, Jacobs AA, McConnell SK. Tangential migration of neurons in the developing cerebral cortex. Development 1995;121:2165–76. Kim Y-t, Haftel VK, Kumar S, Bellamkonda RV. The role of aligned polymer ﬁber-based constructs in the bridging of long peripheral nerve gaps. Biomaterials 2008;29:3117–27. Schmidt CE, Leach JB. Neural tissue engineering: strategies for repair and regeneration. Annu Rev Biomed Eng 2003;5: 293–347. Xie J, MacEwan MR, Schwartz AG, Xia Y. Electrospun nanoﬁbers for neural tissue engineering. Nanoscale 2010;2:35–44. Wang W, Itoh S, Konno K, Kikkawa T, Ichinose S, Sakai K, Ohkuma T, Watabe K. Effects of Schwann cell alignment along the oriented electrospun chitosan nanoﬁbers on nerve regeneration. J Biomed Mater Res, A 2009;91:994–1005. Wang W, Itoh S, Yamamoto N, Okawa A, Nagai A, Yamashita K. Enhancement of nerve regeneration along a chitosan nanoﬁber mesh tube on which electrically polarized ␤-tricalcium phosphate particles are immobilized. Acta Biomater 2010;6:4027–33.
 Koh H, Yong T, Teo W, Chan C, Puhaindran M, Tan T, Lim A, Lim B, Ramakrishna S. In vivo study of novel nanoﬁbrous intra-luminal guidance channels to promote nerve regeneration. J Neural Eng 2010;7 (046003/1-14).  Wakelam M. The fusion of myoblasts. Biochem J 1985;228:1–12.  Aviss K, Gough J, Downes S. Aligned electrospun polymer ﬁbres for skeletal muscle regeneration. Eur Cell Mater 2010;19: 193–204.  Cooper A, Jana S, Bhattarai N, Zhang M. Aligned chitosanbased nanoﬁbers for enhanced myogenesis. J Mater Chem 2010;20:8904–11.  Shin S-H, Purevdorj O, Castano O, Planell JA, Kim H-W. A short review: recent advances in electrospinning for bone tissue regeneration. J Tissue Eng 2012;3:11 (2041731412443530).  Lyu S, Huang C, Yang H, Zhang X. Electrospun ﬁbers as a scaffolding platform for bone tissue repair. J Orthop Res 2013;31:1382–9.  Rim NG, Shin CS, Shin H. Current approaches to electrospun nanoﬁbers for tissue engineering. Biomed Mater 2013;8:1–14.  Zhang Z, Hu J, Ma PX. Nanoﬁber-based delivery of bioactive agents and stem cells to bone sites. Adv Drug Deliv Rev 2012;64:1129–41.  Schofer MD, Roessler PP, Schaefer J, Theisen C, Schlimme S, Heverhagen JT, Voelker M, Dersch R, Agarwal S, Fuchs-Winkelmann S, Paletta JR. Electrospun PLLA nanoﬁber scaffolds and their use in combination with BMP-2 for reconstruction of bone defects. Plos One 2011;6:1–9.  Laurencin CT, Ashe KM, Henry N, Kan HM, Lo KW-H. Delivery of small molecules for bone regenerative engineering: preclinical studies and potential clinical applications. Drug Discov Today 2014;19:794–800.  Wright L, McKeon-Fischer K, Cui Z, Nair L, Freeman J. PDLA/PLLA and PDLA/PCL nanoﬁbers with a chitosan-based hydrogel in composite scaffolds for tissue engineered cartilage. J Tissue Eng Regen Med 2012:9, http://dx.doi.org/10.1002/term.1591.  Son YJ, Kim WJ, Yoo HS. Therapeutic applications of electrospun nanoﬁbers for drug delivery systems. Arch Pharm Res 2014;37:69–78. ˜  Chatakun P, Núnez-Toldrà R, López ED, Gil-Recio C, Martínez-Sarrà E, Hernández-Alfaro F, Ferrés-Padró E, Giner-Tarrida L, Atari M. The effect of ﬁve proteins on stem cells used for osteoblast differentiation and proliferation: a current review of the literature. Cell Mol Life Sci 2014;71:113–42.  Lieberman JR, Daluiski A, Einhorn TA. The role of growth factors in the repair of bone biology and clinical applications. J Bone Joint Surg 2002;84:1032–44.  Urist MR. Bone: formation by autoinduction. Science 1965;150:893–9.  Bessa PC, Casal M, Reis R. Bone morphogenetic proteins in tissue engineering: the road from laboratory to clinic, Part II (BMP delivery). J Tissue Eng Regen Med 2008;2:81–96.  Lo KW-H, Ulery BD, Ashe KM, Laurencin CT. Studies of bone morphogenetic protein-based surgical repair. Adv Drug Deliv Rev 2012;64:1277–91.  Lo KW, Ashe KM, Kan HM, Laurencin CT. The role of small molecules in musculoskeletal regeneration. Regen Med 2012;7:535–49.  Li C, Vepari C, Jin H-J, Kim HJ, Kaplan DL. Electrospun silk-BMP-2 scaffolds for bone tissue engineering. Biomaterials 2006;27:3115–24.  Casper CL, Yamaguchi N, Kiick KL, Rabolt JF. Functionalizing electrospun ﬁbers with biologically relevant macromolecules. Biomacromolecules 2005;6:1998–2007.  Kuihua Z, Chunyang W, Cunyi F, Xiumei M. Aligned SF/P (LLA-CL)-blended nanoﬁbers encapsulating nerve growth factor for peripheral nerve regeneration. J Biomed Mater Res, A 2014;102:2680–91.  Manning C, Schwartz A, Liu W, Xie J, Havlioglu N, Sakiyama-Elbert S, Silva MJ, Xia Y, Gelberman RH, Thomopoulos S. Controlled delivery of mesenchymal stem cells and growth factors using a nanoﬁber scaffold for tendon repair. Acta Biomater 2013;9:6905–14.  Xie Z, Paras CB, Weng H, Punnakitikashem P, Su L-C, Vu K, Tang L, Yang J, Nguyen KT. Dual growth factor releasing multi-functional nanoﬁbers for wound healing. Acta Biomater 2013;9:9351–9.  Ferrand A, Eap S, Richert L, Lemoine S, Kalaskar D, DemoustierChampagne S, Atmani H, Mély Y, Fioretti F, Schlatter G, Kuhn L, Ladam G, Benkirane-Jessel N. Osteogenetic properties of electrospun nanoﬁbrous PCL scaffolds equipped with chitosan-based nanoreservoirs of growth factors. Macromol Biosci 2014;14: 45–55.  Neal RA, Tholpady SS, Foley PL, Swami N, Ogle RC, Botchwey EA. Alignment and composition of laminin–polycaprolactone
T. Jiang et al. / Progress in Polymer Science 46 (2015) 1–24 nanoﬁber blends enhance peripheral nerve regeneration. J Biomed Mater Res, A 2012;100:406–23. Junka R, Valmikinathan CM, Kalyon DM, Yu X. Laminin functionalized biomimetic nanoﬁbers for nerve tissue engineering. J Biomater Tissue Eng 2013;3:494–502. Liu JJ, Wang CY, Wang JG, Ruan HJ, Fan CY. Peripheral nerve regeneration using composite poly(lactic acid-caprolactone)/nerve growth factor conduits prepared by coaxial electrospinning. J Biomed Mater Res, A 2011;96:13–20. Selcan Gungor-Ozkerim P, Balkan T, Kose GT, Sezai Sarac A, Kok FN. Incorporation of growth factor loaded microspheres into polymeric electrospun nanoﬁbers for tissue engineering applications. J Biomed Mater Res, A 2014;102:1897–908. Lo WHK, Ulery D, Deng BM, Ashe MK, Laurencin TC. Current patents on osteoinductive molecules for bone tissue engineering. Recent Pat Biomed Eng 2011;4:153–67. Laurencin CT, Lo K. Bone morphogenetic proteins for bone regeneration and their alternatives. Curr Pharm Des 2013;19: 3353–63. Blaich G, Janssen B, Roth G, Salfeld J. Overview: differentiating issues in the development of macromolecules compared with small molecules. In: Gad SC, editor. Handbook of pharmaceutical biotechnology. Hoboken, NJ: John Wiley & Sons Inc; 2007. p. 89–123. Reid RC, Yau M-K, Singh R, Hamidon JK, Reed AN, Chu P, Suen JY, Stoermer MJ, Blakeney JS, Lim J, Faber JM, Fairlie DP. Downsizing a human inﬂammatory protein to a small molecule with equal potency and functionality. Nat Commun 2013;4:1–9. Mieszawska AJ, Kaplan DL. Smart biomaterials-regulating cell behavior through signaling molecules. BMC Biol 2010;8:1–3. Siddappa R, Martens A, Doorn J, Leusink A, Olivo C, Licht R, van Rijn L, Gaspar C, Fodde R, Janssen F, van Blitterswijk C, de Boer J. cAMP/PKA pathway activation in human mesenchymal stem cells in vitro results in robust bone formation in vivo. Proc Nat Acad Sci USA 2008;105:7281–6. Siddappa R, Mulder W, Steeghs I, van de Klundert C, Fernandes H, Liu J, Arends R, van Blitterswijk C, de Boer J. cAMP/PKA signaling inhibits osteogenic differentiation and bone formation in rodent models. Tissue Eng, A 2009;15:2135–43. Lo KWH, Kan HM, Ashe KM, Laurencin CT. The small molecule PKA-speciﬁc cyclic AMP analogue as an inducer of osteoblast-like
  
cells differentiation and mineralization. J Tissue Eng Regen Med 2012;6:40–8. Lo KWH, Kan HM, Gagnon KA, Laurencin CT. One-day treatment of small molecule 8-bromo-cyclic AMP analogue induces cell-based VEGF production for in vitro angiogenesis and osteoblastic differentiation. J Tissue Eng Regen Med 2013, http://dx.doi.org/10.1002/term.1839/1-9. Kouhi M, Morshed M, Varshosaz J, Fathi MH. Poly(-caprolactone) incorporated bioactive glass nanoparticles and simvastatin nanocomposite nanoﬁbers: preparation, characterization and in vitro drug release for bone regeneration applications. Chem Eng J 2013;228:1057–65. Singh H, James E, Kan H-M, Nair LS. Fabrication and evaluation of resveratrol loaded polymeric nanoﬁbers. J Biomater Tissue Eng 2012;2:228–35. Das A, Segar CE, Hughley BB, Bowers DT, Botchwey EA. The promotion of mandibular defect healing by the targeting of S1P receptors and the recruitment of alternatively activated macrophages. Biomaterials 2013;34:9853–62. Rishton GM. Small molecules that promote neurogenesis in vitro. Recent Pat CNS Drug Discov 2008;3:200–8. Teo W, Ramakrishna S. A review on electrospinning design and nanoﬁbre assemblies. Nanotechnology 2006;17:R89–106. Whited BM, Whitney JR, Hofmann MC, Xu Y, Rylander MN. Pre-osteoblast inﬁltration and differentiation in highly porous apatite-coated PLLA electrospun scaffolds. Biomaterials 2011;32:2294–304. Keun Kwon I, Kidoaki S, Matsuda T. Electrospun nano-to microﬁber fabrics made of biodegradable copolyesters: structural characteristics, mechanical properties and cell adhesion potential. Biomaterials 2005;26:3929–39. Liu W, Yeh Y-C, Lipner J, Xie J, Sung H-W, Thomopoulos S, Xia Y. Enhancing the stiffness of electrospun nanoﬁber scaffolds with a controlled surface coating and mineralization. Langmuir 2011;27:9088–93. Zhou X, Cai Q, Yan N, Deng X, Yang X. In vitro hydrolytic and enzymatic degradation of nestlike-patterned electrospun poly(d,l-lactide-co-glycolide) scaffolds. J Biomed Mater Res, A 2010;95:755–65.